Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Document related concepts

Maxwell's equations wikipedia, lookup

Electrical resistivity and conductivity wikipedia, lookup

Electromagnetism wikipedia, lookup

Electromagnet wikipedia, lookup

Partial differential equation wikipedia, lookup

Navier–Stokes equations wikipedia, lookup

Time in physics wikipedia, lookup

Electrical resistance and conductance wikipedia, lookup

Superconductivity wikipedia, lookup

Turbulence wikipedia, lookup

Transcript
```PHYSICAL REVIEW B
VOLUME 62, NUMBER 6
1 AUGUST 2000-II
Nonlinear transport current flow in superconductors with planar obstacles
Alex Gurevich and Mark Friesen
Applied Superconductivity Center, University of Wisconsin, Madison, Wisconsin 53706

We present a detailed description of a hodograph method, which enables us to calculate analytically the
two-dimensional distributions of the electric field E(r) and transport current density J(r) in superconductors,
taking into account their highly nonlinear E-J characteristics. The method gives a unique solution E(r) of
nonlinear steady-state Maxwell’s equations for given boundary conditions, showing applicability limits of the
critical state model and pointing out where it breaks down. The nonlinear problem of calculation of J(r) by the
hodograph method reduces to solving a linear equation for the electric potential ␸ (E), or the current stream
function ␺ (E) as a function of E. For the power-law characteristics E⫽E c (J/J c ) n , calculation of E(r) and
J(r) can be mapped onto solutions of the London equation with the inverse screening length ␤ ⫽(n
⫺1)/2冑n in the hodograph space (E x E y ). We give general methods of solving the hodograph equations and
obtain closed-form analytical solutions for particular current flows. The method is applied to calculate distributions of E(r) and dissipation in superconductors with macroscopic planar defects, such as high-angle grain
boundaries, microcracks, etc. Current patterns around planar obstacles are shown to break up into domains of
different orientations of J, separated by current domain walls. We calculate the structure of the current domain
walls, whose width depends both on the geometry of current flow and the exponent n. These domain walls
differ from the current discontinuity lines of the Bean model even in the limit n→⬁. We obtained a solution
for current flow past a planar defect of length 2a in an infinite superconductor and showed that the defect
causes strong local electric-field enhancement and long-range disturbances of E(r) on length scales L⬜ ⬃an
Ⰷa and L 储 ⬃a 冑nⰇa perpendicular and parallel to the mean current flow, respectively. This solution also
exhibits large stagnation regions of magnetic flux near planar defects, universal distributions of J(r) in the
critical state limit, n→⬁, and local flux flow regions near the edges. We calculate Joule heating for nonlinear
current flow and show that planar defects cause significant excess dissipation, which affects ac losses and local
thermal instabilities in superconductors.
I. INTRODUCTION
Macroscopic electrodynamics of type-II superconductors
in the mixed state is determined by the pinning and thermally
activated creep of vortex structures, which gives rise to a
weakly dissipative critical current, irreversible magnetization, and slow current relaxation 共flux creep兲. These phenomena manifest themselves on length scales much larger than
the Larkin pinning correlation length L c , on which the critical state is formed.1 On these macroscopic scales LⰇL c , the
only material characteristic which determines the behavior of
superconductors in electromagnetic fields is the nonlinear local relation between the electric field E and current density J,
J⫽
E
J共 E 兲.
E
enable one to calculate the evolution of nonuniform distributions of E(r,t) and B(r,t) and thus to describe macroscopic
magnetic, transport, and relaxation phenomena in
superconductors.1–4
A type-II superconductor in the mixed state exhibits a
highly nonlinear E(J) dependence below a critical current
density J c , which separates regimes of flux flow at J⬎J c
and flux creep at J⬍J c 共Fig. 1兲. The crucial behavior of
E(J) at J⬍J c is determined by thermally activated vortex
creep:

E 共 J 兲 ⫽E c exp ⫺

U 共 J,T,B 兲
,
T

Here E(r,t) and J(r,t) refer to the macroscopic electric field
and current density averaged over all relevant intrinsic scales
of pinned vortex structure, such as intervortex spacing, pinning correlation lengths, etc. We consider an isotropic E-J
relation 共1兲, which, for example, models the nearly twodimensional 共2D兲 current flow in the ab plane of layered
high-temperature superconductors 共HTS’s兲. Equation 共1兲,
combined with the Maxwell equations
⳵ t B⫽⫺ⵜ⫻E,
ⵜ⫻H⫽J共 E兲 ,
0163-1829/2000/62共6兲/4004共22兲/\$15.00

PRB 62
FIG. 1. E-J characteristic of a type-II superconductor.
4004
PRB 62
NONLINEAR TRANSPORT CURRENT FLOW IN . . .
4005
FIG. 2. Percolative current flow in polycrystals. Currentblocking high-angle grain boundaries are shown as solid lines,
while low-angle grain boundaries, transparent to current flow, are
shown as dashed lines.
where U(J,T,B) is an activation barrier, which depends on
J, the temperature T, and the magnetic induction, B. Here E c
is a conditional electric-field criterion, which defines an apparent J c by the relation, U(J c ,T,B)⫽0. For instance, vortex glass/collective creep models1 give a divergent dependence U⫽U c 关 (J c /J) ␮ ⫺1 兴 at small JⰆJ c , which has been
observed in transport and magnetization measurements on
HTS’s.3 Similar though less singular logarithmic dependence
U⫽U c ln(Jc /J) corresponds to power-law E-J characteristics, E⫽E c (J/J c ) n with n(T,B)⫽U c /T⬃3 –30. It is a good
approximation of the observed E(J) for type-II superconductors, especially for layered Bi-based HTS’s.5
If the distribution of J(r) varies on spatial scales greater
than L c , a superconductor can be regarded as a highly nonlinear, nonuniform conductor with a local characteristic
E(J,r). For example, Eqs. 共1兲 and 共2兲 describe nonlinear
transport in superconductors with macroscopic obstacles or
percolative current flow in HTS polycrystals with grain sizes
ⰇL c 共Fig. 2兲. This case is important for understanding
current-limiting mechanisms of HTS’s, which, in addition to
grain boundaries, often contain other macroscopic defects,
such as second phase precipitates, microcracks, and regions
of local nonstoichiometry on scales of order 10–1000 ␮ m.6
These current-blocking obstacles cause macroscopically nonuniform distributions of transport and magnetization currents, as revealed by magneto-optical imaging of HTS’s.7–10
In turn, even comparatively weak inhomogeneities of local
J(r) can cause exponentially strong variations of the electric
field, E(r)⬀J exp关⫺U(J)/T兴, which radically change global
characteristics of superconductors J̄(Ē,B,T) observed in experiment. Thus the behavior of J̄(Ē,B,T) can be different
from local characteristics 共1兲 determined by thermally activated vortex dynamics and pinning on mesoscopic scales,
L⬍L c . For instance, the relation between global J̄(Ē,B,T)
characteristics and local J(E,r) is rather complex, even in
nonuniform Ohmic conductors.11 This is even more so for
superconductors, where the global and local characteristics
can exhibit different dependencies on E, B, and T, because
the nonlinearity of E(J) makes the effective current-carrying
cross section dependent on T, B, and E.12–15
Shown in Fig. 3 are examples of 2D current flows for
different cases, which could be regarded as elementary
‘‘building blocks’’ of a more general percolative network in
Fig. 2. The geometries shown in Fig. 3 are also quite common in experimental studies of resistive states in supercon-
FIG. 3. Characteristic cases of the 2D nonlinear current flow
solvable by the hodograph method.
ductors, thin-film superconducting electronic circuits and
HTS conductors for power applications. For instance, Fig.
3共a兲 shows a superconducting film with a strong currentlimiting planar defect 共microcrack or high angle grain
boundary兲. The case in Fig. 3共a兲 is also mathematically
analogous to that in Fig. 3共b兲, which shows current flow
through a faceted grain boundary with alternating segments
of different J c values. Other common geometries include the
current injector 共or magnetic flux transformer兲 关Fig. 3共c兲兴 and
the microbridge 关Fig. 3共d兲兴. In all cases shown in Figs. 2 and
3, the electric field and current density are inhomogeneous
on macroscopic scales and have singularities near the sharp
edges and corners. Calculations of the global E-J characteristics then require solving Eqs. 共1兲 and 共2兲.
The highly nonlinear Eqs. 共1兲 and 共2兲 represent a difficult
mathematical problem, which has, to our knowledge, not so
far been addressed analytically, except for a few results on
1D flux penetration16 and flux creep dynamics.4 Extensive
numerical studies of the dynamics of flux penetration by
Brandt17 have revealed many important features of nonlinear
flux dynamics in superconductors, such as narrow domain
walls separating regions with different directions of current
flow, nonlocal flux diffusion in thin samples, the influence of
geometrical barrier, etc. On the other hand, the problem of
2D steady-state transport current flow has remained unsolved, because even numerical simulations of Eqs. 共1兲 and

of E(J) increases. For large n values, even weak spatial
variations of J(r) around planar defects in Fig. 2 produce
exponentially large variations of electric field E(r)
⫽E c 关 J(r)/J c 兴 n . This fact along with singularities of J(r)
and E(r) at the edges considerably complicate numerical
analysis of Eqs. 共1兲 and 共2兲, making it necessary to develop
an analytical method for solving Eqs. 共1兲 and 共2兲.
An approximate method for obtaining current distribution
in superconductors is given by the Bean critical state
model,18,19 which replaces the real E(J) curve 共1兲 by a stepwise dependence: J⫽EJ c /E for E⬎0, and E⫽0 for J⬍J c

the power-law characteristic, E⫽E c (J/J c ) n for n→⬁,17
which enables analytical solutions for J(r) for some simple
cases 共Fig. 4兲. These solutions exhibit characteristic ‘‘discon-
4006
ALEX GUREVICH AND MARK FRIESEN
PRB 62
the infinite extent of current perturbations around local inhomogeneities 共Fig. 4兲, the zero thickness of the d lines, and
multiple solutions of the Bean model, fixing a unique steadystate transport current distribution for given boundary conditions. However, the account of the nonlinear E(J) requires
solving the following nonlinear equation for the scalar potential ␸ :

div
FIG. 4. Magnetization current flows predicted by the Bean
model. Top: long slab in a parallel magnetic field. Bottom: current
flow around a cylindrical void 共Ref. 19兲. Dashed lines show the
parabolic d lines, on which J sharply changes direction. Current
streamlines between the d lines are circular, and centered in the
void.
tinuity’’ lines (d lines兲, along which the current abruptly
changes direction. Another feature of this model is that
finite-size defects can cause current disturbances of infinite
range, as it occurs for current flow past a cylindrical void, in
which case parabolic d lines extend to infinity19,20 关Fig. 4共b兲兴.
Both the zero thickness of the d lines and the infinite spatial
scale of current perturbations are consequences of the zero
resistivity for the idealized Bean’s E-J characteristic in the
whole interval 0⬍J⭐J c . In this case, solving steady-state
Eqs. 共2兲 becomes an ill-defined mathematical problem,
which reduces to the only condition of current continuity,
div J⫽0, provided that J⭐J c . These conditions can be satisfied by many different current distributions for a given
sample geometry, since the selection of Bean’s solutions for
J(r) is due to initial conditions. For example, the initial distribution of electric field E(r) can be induced by increasing
external magnetic field. Once the initial conditions are fixed
by the magnetic prehistory, the distribution of J(r) stays
frozen indefinitely.
The inherent hysteresis of the critical state makes the
Bean model inappropriate for calculations of steady-state
transport current flow around planar obstacles in Figs. 2 and
3, for which the current-carrying cross section varies along a
superconductor. In this case current path inevitably breaks
into regions in the critical state, J⫽J c , and subcritical regions, with 0⬍J⬍J c . However, the particular distribution
of these regions depends on initial conditions and thus cannot be calculated by solving the steady-state equations,
div J⫽0 and J⭐J c . This unphysical situation results from
the fact that the Bean model ignores the necessary condition
ⵜ⫻E⫽0, which can only be satisfied by taking account of
the highly nonlinear E-J characteristics 共1兲. Although exponentially small at J⬍J c , the nonzero electric field plays an
important role, since solving Eqs. 共1兲 now becomes a welldefined mathematical problem, for which each nonzero value
of J corresponds to a certain E. The account of E eliminates

ⵜ␸
J 共 兩 ⵜ ␸ 兩 兲 ⫽0,

which is obtained by substituting E⫽⫺ⵜ ␸ into Eq. 共1兲 and
then into div J⫽0. The 2D Eq. 共4兲 is rather difficult to solve
either analytically or numerically.
Recently we proposed an analytical method to calculate
2D steady-state transport current flow in superconductors
with the account of their nonlinear E(J) characteristics.21,22
The method is based on a hodograph transformation, developed at the beginning of the 20th century to describe compressible gas flow.23,24 In Ref. 21 the hodograph method was
developed as to describe current flow in anisotropic superconductors. Using this method, analytical steady-state solutions of Eqs. 共1兲 and 共2兲 for current flow past a planar defect
were obtained for the power-law E-J characteristics.22 The
essence of the hodograph method is the following. Instead of
dealing with the highly nonlinear equation for ␸ (r) in the
coordinate space, we change variables and express ␸ (r) as a
function of the electric field E:
␸ 共 r兲 → ␸ 共 E兲 .

The hodograph transformation 共5兲 reduces the nonlinear Eq.

linear partial differential equations, such as Thomas-Fermi or
London equations, whose known solutions can be used to
obtain exact solutions for 2D current flows in nonlinear conductors. For example, the nonlinear current flow around a
planar defect can be mapped onto a solution of the London
equation, which describes the magnetic-field distribution
from a fictitious fluxon in a film with cuts. Here the nonlinearity of the power-law characteristic E⫽E c (J/J c ) n manifests itself in the nonzero effective ‘‘screening length’’ l
⫽2 冑n/(n⫺1). These analogies enables one to use known
solutions of the London, Debye, or diffusion equations 共see
below兲 to obtain analytical solutions for the 2D nonlinear
current flows in superconductors with macroscopic defects.22
The hodograph method enables us to resolve the ambiguities of the Bean model and address analytically features of
2D nonlinear transport current flow. In particular, it gives a
unique steady-state distribution J(r) for a given sample geometry and shows that current flow breaks into domains with
different orientations of J separated by current domain walls
reminiscent of the d lines of the Bean model. However, there
are important differences between the current domain walls
and the d lines. First of all, the domain walls have an internal
structure and a varying width, which depends both on the n
value and the geometry of current flow. For instance, for
current flow past a void in Fig. 4, the width of the domain
PRB 62
NONLINEAR TRANSPORT CURRENT FLOW IN . . .
walls increases with the distance from the void. It is the
broadening of the domain walls, which provides the decay of
current perturbations caused by the defect size a on a finite
length L⬜ ⬃an, much larger than a, if nⰇ1. Moreover, the
current domain walls described by exact hodograph solutions
remain different from the phenomenological d lines even in
the critical state limit, n→⬁. In this case current flow near
domain walls exhibits no discontinuities in the tangential
components of J(x,y) thus satisfying ⵜ⫻E⫽0.
In this and a subsequent paper25 we present a detailed
description of the hodograph method and calculate various
steady-state 2D transport current flow in superconductors. In
this paper we focus on general features of current flow in
isotropic nonlinear conductors illustrated by characteristic
examples, which show how the method works. We present
exact solutions of Eq. 共4兲, which reveal new length scales of
nonlinear current flow and the structure of current domain
walls. The second part of this work25 is devoted to calculations of the distributions of J(r) and E(r) for restricted geometries shown in Fig. 3. Because of the long-range disturbances of the E(x,y) near defects in superconductors,22 the
effect of the sample geometry becomes crucial and in many
cases completely dominates the global nonlinear current
transport. These results enable us to calculate global E-J
characteristics and dissipation due to defects, which also pertain to the problems of current-carrying capability, ac losses,
and thermal stability of superconductors. In addition to superconductors, the hodograph method can also be applied to
calculations of nonuniform current flow in other nonlinear
media, such as semiconductors, plasma, etc. For instance,
E-J characteristics of gas or semiconductor plasma at high
electric fields can be approximated by the power-law dependence, E⬀J n , with nⰆ1.26
The paper is organized as follows. In Sec. II we consider
features of nonlinear current flow and discuss conditions,
under which the steady-state current distributions in superconductors set in. In Sec. III we formulate the hodograph
method and give general solutions of the hodograph equations, which then will be used to reveal features of the 2D
current flows for particular geometries. In Sec. IV we consider current flow past a semi-infinite corner and calculate
analytically the structure of the current domain walls and
singularities in J(r) and E(r) distributions near sharp edges.
In Sec. V we obtain a solution for current flow past a nonconducting planar defect in an infinite superconductor, and
identify the new length scales of E(r) which are caused by
the nonlinearity of E(J). We describe flux flow regions near
the edge of the planar defect and address a nontrivial critical
state limit at n→⬁. In Sec. VI we calculate excess dissipation on planar defects for nonlinear E(J) characteristics. Sec.
VII is devoted to the discussion of the results and their implications for nonlinear current transport and current-limiting
mechanisms in HTS’s.
II. NONLINEAR 2D CURRENT FLOW
A. Time scales
In this paper we consider the 2D steady-state transport
current flow, which sets in after initial relaxation of current
distribution induced by switching on a dc power supply. In
superconductors, such transient processes can dominate the
4007
observable behavior on ‘‘human’’ time scales, because the
strong nonlinearity of J(E) can make the relaxation time t 0
astronomically large. In this case, the superconductor remains in a metastable critical state, which relaxes very
slowly toward a true steady state. Therefore an estimation of
t 0 is necessary to find the conditions, under which the
We estimate t 0 of macroscopic current relaxation, assuming that a superconductor is in a high magnetic field, so that
both self-field effects and the surface or geometrical barriers
can be neglected. In this case ␮ 0 H⫽B, and J(E,B)
⫽J(E,B 0 ), where B 0 / ␮ 0 is a constant applied magnetic
field. Eqs. 共2兲 then reduce to
␮ 0 ␴⳵ t E⫽⫺ⵜ⫻ⵜ⫻E.

Here ␴ (E)⫽ ⳵ J/ ⳵ E is the differential conductivity, whose
dependence on E⫽ 兩 E兩 determines the dynamics of E(r,t).
The important feature of ␴ (E) in the subcritical state (E
ⰆE c ) is an approximately inverse dependence ␴ (E)
⬇J 1 /E for all existing models of thermally activated vortex
dynamics described by Eq. 共1兲.4 This universality holds in a
very wide region of E to the accuracy of a much weaker
logarithmic variation of J 1 (E) at large n⬃3 –30. Here the
parameter J 1 ⫽T/ 兩 ⳵ J U 兩 ⫽sJ can be expressed in terms of the
observed dimensionless flux creep rate, s⫽d ln J/d ln t.1–4
Since macroscopic electrodynamics of superconductors
becomes model independent, when formulated in terms of
the electric field E(r,t), the time scale t 0 can be estimated by
a scaling analysis of Eq. 共6兲.4 Indeed, Eq. 共6兲 can be regarded
as a nonlinear diffusion equation for the electric field E with
the diffusivity D(E)⫽1/␮ 0 ␴ . Thus the time scale t 0 of current redistribution in a region of size L is given by t 0
⬃L 2 /D, whence
t 0 ⬃ ␮ 0 L 2 J 1 /E.

Here t 0 determines the duration of a transient process after
which a steady-state current flow sets in. Because of the
exponential dependence of E on J, the electric field E in Eq.

The upper bound of t 0 can be estimated by substituting the
steady-state E(r) in Eq. 共7兲. For instance, taking the standard
electric field criterion, E c ⯝1 ␮ V/cm for J c and a characteristic spacing between defects, L⯝100 ␮ m, we obtain t 0
⯝0.06 sec, for J 1 ⫽sJ c , J c ⫽106 A/cm2 and s⫽0.05. In this
case a steady-state transport current flow sets in on a short
time scale, even for high J c values.
However, geometrical constraints for certain sample geometries can make t 0 much larger than the above estimate.
As an example, we first consider the current lead of width L 1
attached to a sample of width L 2 ⬎L 1 关Fig. 3共c兲兴, assuming
the power law E⫽E c (J/J c ) n with n⯝3 –20. Let the lead be
in a uniform critical state, (E 1 ⯝E c ), which sets in at t⬎t 1
⯝ ␮ 0 sJ c L 21 /E c . Then it takes t⬎t 2 ⯝ ␮ 0 sJ c L 22 /E 2 for a
steady-state uniform current flow to occur in the sample,
where E 2 is determined by the current conservation condition, E 2 ⫽E 1 (L 1 /L 2 ) n , giving t 2 ⯝t 1 (L 2 /L 1 ) n⫹2 . For n
⫽15 and L 2 ⫽2L 1 , this yields t 2 ⯝1.3⫻105 t 1 , or about 2.2 h
for t 1 ⫽0.06 sec.
A similar argument can be made for the important case of
a planar defect in a film 关Fig. 3共a兲兴, for which L 2 ⫽d, L 1
4008
ALEX GUREVICH AND MARK FRIESEN
⯝d⫺a, where d is the film thickness, and a is the length of
the defect. If the electric field near defect is of order E c , then
the electric field in the bulk, E 2 ⯝(1⫺a/d) n E 1 can be much
smaller than E c , even for a small defect, aⰆd. Thus the
steady-state current flow near defect sets in after t⬎t 1
⯝ ␮ 0 sJ c (d⫺a) 2 /E c , while it can take a much longer time,
t⬎t 2 ⬃t 1 /(1⫺a/d) n⫹2 in the bulk. For d⫽1 mm, n⫽15,
J 1 ⫽5⫻104 A/cm2 , we find that t 1 ⯝6.3 sec, but t 2 ⬃38 sec
for a⫽0.1d, t 2 ⬃45 min for a⫽0.3d, and t 2 ⬃9.6 days for
a⫽0.5d. For larger a and n, relaxation toward a steady-state
transport current distribution occurs on time scales well exceeding the experimental time window.
The above examples show that, although the transient relaxation of J(r,t) could be very slow for certain geometries,
the steady-state transport current flow for the most cases discussed in the Introduction sets in on rather short time scales.
Such relaxation is accelerated in HTS’s, where flux creep is
rather fast, and the n values are significantly smaller than in
low-T c superconductors.3 In the rest of this paper we therefore consider the nonlinear steady-state 2D transport current
flow in superconductors, disregarding the transient period t
⬍t 0 , on which steady-state E(x,y) is formed. The relevant
time scales t 0 can be estimated from Eq. 共7兲 for any steadystate distribution E(x,y).
For steady-state current flow, Eqs. 共2兲 become
ⵜ⫻E⫽0,
ⵜ⫻H⫽J.

To satisfy the conditions div J⫽0 and ⵜ⫻E⫽0, for the 2D
current flow in the xy plane, we introduce the scalar potential
␸ and the stream function ␺ , related to J and E as follows:
J x⫽ ⳵ y␺ ,
E x ⫽⫺ ⳵ x ␸ ,
J y ⫽⫺ ⳵ x ␺ ,

E y ⫽⫺ ⳵ y ␸ ,

where ⳵ ␣ ⬅ ⳵ / ⳵ ␣ . The magnetic field H(r) is expressed in
terms of ␺ (x ⬘ ,y ⬘ ) by the Bio-Savart law,
H共 r兲 ⫽
1
2␲

V

d 3 r⬘ ,

where the integral is taken over the current flow regions, and
n̂ is the unit vector along the z axis. The stream function ␺
coincides with the normal component of the magnetic field
H n for the 2D current flow in a long cylinder or slab, but can
be very different from H n for thin films.27–31 For Ohmic
conductors, both ␸ and ␺ satisfy the Laplace equation ⵜ 2 ␸
⫽0, ⵜ 2 ␺ ⫽0, so it is convenient to introduce the complex
potential w(z)⫽ ␸ ⫺i ␳ ␺ , which is an analytic function of the
complex coordinate z⫽x⫹iy. Here ␳ ⫽E/J, and the real and
imaginary parts of w(z) obey the boundary conditions for ␸
and ⫺ ␳ ␺ , respectively. This fact enables one to use powerful methods of the theory of analytic functions to calculate
the 2D transport current flow in Ohmic conductors.32 This
technique is also useful for calculation of magnetization currents in superconductors.27–29
PRB 62
In nonlinear conductors the situation is much more complicated, since w(z) is no longer analytic function. As a result, nonlinear current flow generally causes bulk charge
density distribution, q⫽div E,
q⫽ 共 ⳵ J ␳ 兲 JⵜJ,

since the resistivity ␳ ⫽E/J now depends on J. For instance,
for the case shown in Fig. 3共c兲, integration of the charge
density, q⫽div E, gives the total charge accumulated near
the current injector, Q̄⫽(A 1 E 1 ⫺A 0 E 0 ). Here E 1 is the electric field in the injector, and E 0 is the electric field in the
conductor, in regions far away from the joint, where both E 1
and E 0 are uniform, and A 1 and A 0 are the cross-sectional
areas of the injector and the conductor, respectively. For uniform Ohmic conductors, the charge Q̄ vanishes because
A 1 E 1 ⫽A 0 E 0 . By contrast, for nonlinear conductors and A 1
⫽A 0 , we get Q̄⫽0, since A 1 E(I/A 1 )⫽A 0 E(I/A 0 ).
The nonlinearity of E(J) gives rise to new length scales
for the current distribution around a local inhomogeneity. To
show that, we write Eq. 共4兲 in the form
␴ x ⳵ xx ␸ ⫹ ␴ y ⳵ y y ␸ ⫽0,

where ␴ x ⫽ ⳵ J x / ⳵ E x and ␴ y ⫽ ⳵ J y / ⳵ E y are principal values
of the differential conductivity tensor ␴ ik calculated from
Eq. 共1兲:
␴ x ⫽ 共 J/E 兲 sin2 ␪ ⫹ ␴ cos2 ␪ ,

␴ y ⫽ 共 J/E 兲 cos2 ␪ ⫹ ␴ sin2 ␪ .

Here ␴ ⫽ ⳵ J/ ⳵ E is a scalar differential conductivity, and ␪ is
the angle between the direction of the local electric field
E(x,y) and the x axis, so that tan ␪ ⫽E y /E x .
For isotropic Ohmic conductors, the conductivity tensor is
also isotropic, ( ␴ x ⫽ ␴ y ), thus the electric-field perturbations,
␦ E(x,y), decay on a length scale of order the inhomogeneity
size a, both along x and y. However, for any nonlinear isotropic E(J), not only does ␴ ik depend on E, it also becomes
highly anisotropic with respect to the current flow ( ␴ x
⫽ ␴ y ). Assuming that far away from the inhomogeneity, the
current streamlines are nearly parallel to the x axis ( ␪ Ⰶ1),
we obtain that ␴ x ⯝ ⳵ J/ ⳵ E, and ␴ y ⯝J/E. In this case, the
strong nonlinearity of E(J) in superconductors results in
␴ x Ⰶ ␴ y 关for the power-law E⫽E c (J/J c ) n , we have ␴ x
⫽ ␴ y /nⰆ ␴ y 兴. The relation ␴ x Ⰶ ␴ y reflects the fact that the
longitudinal perturbations ␦ E x mostly change the modulus of
J⬇J c , causing a rather weak current response ␦ J x
⫽( ⳵ E J) ␦ E x . By contrast, the transverse perturbations ␦ E y
cause a local turn of the vector Jc , resulting in a much larger
current response ␦ J y ⯝(J c /E) ␦ E y . The fact that ␴ x Ⰶ ␴ y
gives rise to a decay of E(x,y) perturbations over very different length scales L 储 and L⬜ along the x and y axes, respectively. As follows from Eq. 共13兲, we have L⬜
⬃( ␴ y / ␴ x ) 1/2L 储 , whence
L⬜ ⬃L 储 冑n.

This relation will be illustrated below by exact solutions for
particular current flows. Here we just give a simple physical
estimate of L⬜ and L 储 for a planar defect of length 2aⰆd, as
shown in Fig. 3共a兲. The defect blocks current flow on the
PRB 62
NONLINEAR TRANSPORT CURRENT FLOW IN . . .
4009
length ⬃a, forcing the current aJ 0 to redistribute around the
defect on the scale ⬃L⬜ . In the region y⬍L⬜ the mean
current density and the electric field thus increase to J m
⬃(1⫹a/L⬜ )J 0 and E m ⬃(1⫹a/L⬜ ) n E 0 , respectively. The
transverse decay length, L⬜ , is defined by the condition
E m ⬃E 0 , giving L⬜ ⬃na. The decay length, L 储 ⬃a 冑n, along
current flow then follows from Eq. 共16兲. Therefore strong
(nⰇ1) nonlinearity of E(J) greatly increases the spatial
scales of electric-field perturbations, as will be confirmed
below by exact calculations. At the same time, E(x,y) can
also vary on scales much smaller than a, as it occurs in
narrow current domain walls, which replace the sharp d lines
of the Bean model.
In Eq. 共23兲 we can change variables, E⫽E c (J/J c ) n , and express ␺ as a function of E and ␪ , which is convenient for the
further analysis of electric-field distributions. Equations 共23兲
and 共24兲 can also be presented in different useful forms by
introducing new variables,
III. HODOGRAPH TRANSFORMATION
which has the form of the London equation with the inverse
‘‘screening length’’ ␤ :
A. General formalism
Instead of solving the nonlinear Eq. 共13兲, we change variables and take ␸ and ␺ to be functions of the complex electric field E x ⫹iE y ⫽E exp(i␪), where ␪ is the polar angle between E and the x axis. The advantage of such a hodograph
transformation is that it reduces the highly nonlinear Eq. 共13兲
for ␸ (x,y) to linear equations for ␺ (E, ␪ ) and ␸ (E, ␪ ). To
show this we write Eqs. 共8兲 in the differential form,
d ␸ ⫽⫺E x dx⫺E y dy,
␳ d ␺ ⫽E y dx⫺E x dy,

where ␳ (E)⫽E/J. Equations 共17兲 can be combined in a
single complex equation d ␸ ⫺i ␳ d ␺ ⫽⫺Ee ⫺i ␪ dz, whence
⳵ E z⫽⫺e i ␪ 共 ⳵ E ␸ ⫺i ␳⳵ E ␺ 兲 /E,
i␪
⳵ ␪ z⫽⫺e 共 ⳵ ␪ ␸ ⫺i ␳⳵ ␪ ␺ 兲 /E.

Here z⫽x⫹iy is the complex coordinate, and ␴ (E)
⫽ ⳵ J/ ⳵ E is the differential conductivity 共notice that in nonlinear conductors ␳ ⫽1/␴ ). The condition ⳵ ␪2 E z⫽ ⳵ E2 ␪ z then
gives the following relations between partial derivatives of ␺
and ␸ :
⳵ ␪ ␸ ⫽⫺ 共 E 2 /J 兲 ⳵ E ␺ ,
⳵ E ␸ ⫽ 共 E ␴ /J 2 兲 ⳵ ␪ ␺ .

Equating the mixed derivatives, ⳵ ␪2 E ⫽ ⳵ E2 ␪ , for ␺ and ␸ , we
obtain the following linear equations for ␺ and ␸ valid for
any nonlinear dependence J(E):
␴ E ⳵ 2␺
J2 ⳵␪
J ⳵ 2␸
E2 ⳵␪
⫹
2

⳵ E2 ⳵␺
⫽0,
⳵E J ⳵E

⳵ J 2 ⳵␸
⫽0.
⳵E ␴E ⳵E

⫹
2
␸ ⫽e ␤ ␩ h 1 ,
␺ ⫽e ⫺ ␤ ␩ h 2 ,
␩⫽
1

ln
E
.
E0

Here E 0 is the electric field at infinity, and the functions
h 1,2( ␩ , ␪ ) satisfy the equation,
2
2
⳵ ␩␩
h⫹ ⳵ ␪␪
h⫺ ␤ 2 h⫽0,
␤ ⫽ 共 n⫺1 兲 /2冑n.

Therefore the nonlinearity of E(J) results in an effective
screening of ␺ ( ␩ , ␪ ) in the hodograph space, which becomes
stronger as n increases. For n⫽1, Eq. 共26兲 turns into the
Laplace equation, thus the complex potential w(u)⫽ ␸
⫺i ␳ ␺ is an analytic function of u⫽ ␩ ⫺i ␪ in the hodograph
representation. Analytic properties of the complex potential
w( ␩ , ␪ ) in nonlinear conductors are considered in Appendix
A. We show that for n⬎1, w( ␩ , ␪ ) is no longer analytic
function, but can be expressed in terms of generalized analytic functions.33
B. Solving the hodograph equations
The calculation of nonlinear current flow by the
hodograph method is implemented in two steps. First, a solution of the linear Eq. 共21兲 should be found, which satisfies
the particular boundary conditions. Then an inverse transformation of ␺ ( ␪ ,E) from the hodograph plane (E, ␪ ) onto the
physical xy plane should be performed to obtain the current
streamlines ␺ ⫽ ␺ (x,y) and spatial distributions of the electric fields and currents. As shown in Appendix E, the Jacobian of the inverse transformation does not change sign for
any isotropic E-J characteristic with positive differential
conductivity ␴ (E).21 This fact makes the hodograph transformation a well-defined procedure, for which each solution
␺ (E, ␪ ) corresponds to a unique spatial distribution of
E(x,y) for given boundary conditions.
Solutions of Eqs. 共21兲 and 共22兲 can be obtained by separating variables as follows:
␺ 共 E, ␪ 兲 ⫽ 兺 C m f m 共 E 兲 sin共 m ␪ ⫹ ␾ m 兲 .
m

For the power-law dependence, E⫽E c (J/J c ) n , these equations simplify to
Here C m and ␾ m are constants, and the functions f m (E)
satisfy the following ordinary differential equation:
⳵ ␺ ⳵ 2␺
J 2 ⳵ 2␺
⫹
⫹J
⫽0,
n ⳵J2
⳵J ⳵␪2

m 2␴ E
d E2 d f m
⫺
f m ⫽0.
dE J dE
J2

An analogous expression to Eq. 共28兲 for the electric potential
␸ (E, ␪ ) can be obtained with the eigenfunctions g m (E) satisfying
⳵␸ ⳵ 2 ␸
nE
⫹
⫹E
⫽0.
⳵E ⳵␪2
⳵E2
2
⳵ 2␸

4010
ALEX GUREVICH AND MARK FRIESEN

d J 2 dg m
m 2J
⫺ 2 g m ⫽0.
dE ␴ E dE
E

For the power-law J(E) characteristic, Eq. 共23兲 gives
f m (E)⬀E q m , so ␺ (E, ␪ ) takes the form
z⫽z ⫾ ⫹e i ␪
e i␪
⫺
J

PRB 62
B 1 B 2E 0
⫹

J
nE
⬁

m⫽0

⫾
Cm
E
⫾
nq m
⫺1 E 0

⫾
qm
⫾
sin ␽ m 兲 .

␺ 共 E, ␪ 兲 ⫽ ␺ 0 ⫹ 关 B 1 ⫹B 2 共 E/E 0 兲 1/n⫺1 兴共 ␪ ⫹ ␪ 0 兲
⫹
⫾
⫽
qm

⫾
Cm

E
E0
⫾
qm
sin共 m ␪ ⫹ ␾ m 兲 ,
1

2n

Here the sum runs over all integer m, the constants B 1,2 ,
⫾
, ␺ 0 , ␪ 0 , E 0 , and ␾ m are determined by the boundary
Cm
conditions, and E 0 can be taken as the electric field at infinity. We emphasize that Eqs. 共31兲 and 共32兲 are exact general
solutions of the nonlinear Maxwell equations which describe
various current flows.
If distributions E(x,y) contain regions of E⬍E 0 and E
(⫹)
(⫹)
(⫺)
(⫺)
, qm
, and C m
, qm
, the
⬎E 0 , with different sets of C m
solutions ␺ ⫹ (E, ␪ ) for E⬎E 0 and ␺ ⫺ (E, ␪ ) for E⬍E 0
should be matched at E⫽E 0 as to provide continuity of
␺ (E, ␪ ) and its derivatives. Finding the proper relation be(⫹)
(⫺)
and C m
can be reduced to the solution of the
tween C m
following linear matrix equation:25

where U mk and F m are determined by the sample geometry.
The fact that both ␺ ⫺ (E, ␪ ) and ␺ ⫹ (E, ␪ ) are known exactly
is a great advantage of the hodograph method, which thus
reduces the initial nonlinear problem to a standard procedure
of matrix inversion. In some cases the coefficients C m can be
⫺1
F k can be efobtained analytically, otherwise C m ⫽ 兺 k U km
25
fectively calculated numerically. Since the hodograph
method linearizes the Maxwell equations for any E(J), numerical calculations of nonlinear current flow J(x,y) for the
cases shown in Figs. 2 and 3 take no longer than the corresponding calculations of J(x,y) for Ohmic conductors.
The solution 共31兲 is rather convenient for performing the
inverse transformation of ␺ (E, ␪ ) onto the coordinate space
xy, giving the electric-field distribution z⫽z(E, ␪ ) for any
⫾
. This is a well-defined mathematical procedure,
set of C m
since the Jacobian of the inverse transformation is always
positive for any isotropic E-J characteristic, as shown in
Appendix E. To obtain E(x,y), we exclude ⳵ E ␸ and ⳵ ␪ ␸
from Eqs. 共20兲, which yields
⳵ ␪ z⫽
⳵ E z⫽
e i␪

J

␴
e i␪
i ⳵ E␺ ⫺ ⳵ ␪␺ .
J
J
⫾
, and the plus and the
Here z ⫾ are constants, ␽ m ⫽m ␪ ⫹ ␾ m
minus signs correspond to E⬍E 0 and E⬎E 0 , respectively.
Equations 共36兲 represent a complete family of exact solutions of nonlinear Maxwell’s equations for various distributions E(x,y), parameterized by an infinite set of constants
C m . In the following sections we will show how C m can be
found for particular current flows.
Equation 共26兲 belongs to the well-studied linear equation
of mathematical physics, so various nonlinear current distributions can be obtained from known solutions for other
physical problems described by the London or diffusion
equations. For instance, a solution ␺ ( ␩ , ␪ ) of Eq. 共23兲 inside
the region bound by the contour S in the hodograph plane ␩ ␪
can be expressed in terms of the surface distribution ␺ b (s):
␺ 共 ␩ , ␪ 兲 ⫽e ⫺ ␤ ␩

S
e ␤ ␩ ⬘ ␺ b 共 s 兲 ⳵ n G 共 ␩ , ␩ ⬘ , ␪ , ␪ ⬘ 兲 ds. 共37兲
Here ␺ ( ␩ , ␪ ) is determined by the boundary conditions, the
Green’s function G of Eq. 共26兲 satisfies the boundary condition G⫽0 on S, and ⳵ n denotes the normal derivative on S.
The function G has a clear physical meaning, since it is
proportional to the local magnetic field at the point ␩ , ␪ produced by a fictitious London vortex located at the point
␩ ⬘ , ␪ ⬘ in a superconducting cylinder. This analogy enables
one to use extensive results on vortices in superconductors of
different geometries to calculate G( ␩ , ␩ ⬘ , ␪ , ␪ ⬘ ) and thus 2D
current flows in nonlinear conductors.22
Another analogy follows from the following representation of Eqs. 共23兲 and 共24兲:
2
2
⳵ ␪␪
␺ ⫹ ⳵ ␩␩
␺ ⫹2 ␤ ⳵ ␩ ␺ ⫽0,

2
2
⳵ ␪␪
␸ ⫹ ⳵ ␩␩
␸ ⫺2 ␤ ⳵ ␩ ␸ ⫽0.

Equations 共38兲 and 共39兲 have the form of diffusion equations, which describe steady-state distributions of the fields ␺
or ␸ in a reference frame moving with the velocity ⫾2 ␤ .
Equations 共38兲 and 共39兲 also belong to the well-studied linear
equations,34 which could help on finding solutions of the
hodograph equations, using the known solutions of the corresponding diffusion problems. For instance, in the critical
state limit (n→⬁), Eq. 共23兲 becomes a simple 1D diffusion
equation in the hodograph space

⳵ ␶ ␺ ⫽ ⳵ ␪␪ ␺ ,

where ␶ ⫽ln(Jc /J) and ␪ play the roles of ‘‘time’’ and ‘‘coordinate,’’ respectively. In this case the solution of Eq. 共40兲
for the stream function
Substituting Eq. 共31兲 into Eq. 共35兲 and integrating over E, we
obtain
⬁
␺ ⫽B ␪ ⫹ 兺 C m
m⫽1

J
Jc

m2
sin共 m ␪ ⫹ ␾ m 兲

NONLINEAR TRANSPORT CURRENT FLOW IN . . .
PRB 62
4011
flow inside or outside of two unpenetrable walls inclined at
the angle ␣ 共Fig. 5兲. This case allows us to calculate structure of the current domain walls and trace the nonanalytic
crossover from large, but finite n value, to the critical state
limit n→⬁.
A. General solution
The solution for current flow around the corner, satisfies
the boundary conditions, ␺ (E,0)⫽ ␺ (E, ␣ )⫽0, corresponding to zero normal component of J on the sample surface.
This solution of Eq. 共23兲 has the form
␺ ⫽CE q sin k ␪ ,

where k⫽ ␲ /( ␲ ⫺ ␣ ), C is a scaling constant, and
FIG. 5. Inner 共a兲 and outer 共b兲 current flows around a corner.
is independent of n and therefore can be regarded as a ‘‘critical state’’ limit for ␺ (J, ␪ ). However, as will be shown below, Eq. 共41兲 can result in current distributions, which are
different from those of the Bean model.
C. Boundary conditions
To take advantage of the exact solutions for ␺ (E, ␪ ) and
␸ (E, ␪ ), we need to reformulate the corresponding boundary
conditions in the hodograph space. This procedure is rather
nontrivial, since even simple boundary conditions in the xy
plane, such as zero normal component of J on the sample
surface, or a given distribution of J or E on the electrodes,
can become highly nonlinear in the E ␪ plane. For instance, if
current flows past a cylindrical void of radius R, the condition of zero normal component of J(x,y) requires constant
␺ (x,y)⫽ ␺ 0 on the surface, x 2 ⫹y 2 ⫽R 2 . Taking the
hodograph solutions x⫽A(E, ␪ ),y⫽B(E, ␪ ), we obtain the
boundary conditions in the E ␪ plane: A 2 (E, ␪ )⫹B 2 (E, ␪ )
⫽R 2 and ␺ (E, ␪ )⫽ ␺ 0 . Substituting here Eq. 共36兲, we arrive
at an infinite set of coupled nonlinear equations for C m and
␾ m . Therefore the boundary conditions become nonlinear
for curved boundaries or nonuniform distributions of J(x,y)
on the electrodes.
However, for any 2D current flow confined between flat,
piece-wise boundaries, or around planar cuts 共see Figs. 2 and
3兲, the boundary conditions in the hodograph space greatly
simplify. Then the condition of zero normal component of J
at the straight boundary inclined by the angle ␪ 0 becomes
linear, reducing to ␺ (E, ␪ 0 )⫽ ␺ 0 , where ␺ 0 is a constant. For
example, for current flow around a corner shown in Fig. 5,
the boundary conditions can be taken in the form, ␺ (E,0)
⫽ ␺ (E, ␣ )⫽0. Therefore, for current flow around planar obstacles, the hodograph transformation linearizes both the
equation for ␺ (E, ␪ ) and the boundary conditions. In this
case we can obtain complete exact solutions of the nonlinear
Maxwell equations considered in the following sections.
IV. CORNER
One of the simplest exact solutions of Eq. 共23兲 describes
current flow around a corner. There are two different situations which we consider separately, corresponding to current
1

2n
q⫾
k ⫽

Here the plus and the minus signs correspond to current flow
inside and outside the region of the angle ␣ , respectively

we obtain the distribution of E(x,y), substituting Eq. 共42兲
into Eq. 共35兲 and integrating from 0 to E for q⫽q ⫹ and from
⬁ to E for q⫽q ⫺ . This yields
z⫽⫺
Ce i ␪ E q

Separating real and imaginary parts of Eq. 共44兲, and excluding E by dividing y(E, ␪ ) by x(E, ␪ ), we obtain the following equation for the function ␪ (x,y), which determines local
orientation of current flow
y k tan ␪ ⫺nq k tan k ␪
.
⫽
x k⫹nq k tan ␪ tan k ␪

We use these results to consider two particular cases: 共i兲
Current flow past a semi-infinite cut, for which q⫽⫺1, ␣
→0; 共ii兲 Current flow near a rectangular corner, for which
q⫽q ⫾
2 , ␣ ⫽ ␲ /2. In the first case, ␺ ⫽C sin ␪/E is independent of n, and Eq. 共44兲 gives
z⫽
Ce i ␪

Current streamlines described by Eqs. 共42兲 and 共46兲 are
shown in Fig. 6. For nⰇ1, current streamlines are approximately semicircles centered near the end of the cut, while
contours of constant electric field are close to circles which
cross the cut. Near the edge, (x⬇0,y⫽0), the electric field
E(x) has a singularity. For x⬍0 and y→⫾0, currents flow
parallel to the cut 关 ␪ ⫽0 at y⫽⫹0, or ␪ ⫽ ␲ at y⫽⫺0, 共see
Fig. 6兲兴, and Eq. 共46兲 gives x⫽C/(n⫹1)JE. For x⬎0, we
have ␪ ⫽ ␲ /2, and x⫽⫺nC/(n⫹1)JE, whence
E 共 x 兲 ⬀1/nx n/(n⫹1) ,
x⬍0,

E 共 x 兲 ⬀1/x n/(n⫹1) ,
x⬎0.

Hence the circle of constant E of radius R crosses the cut at
the point ⯝R/n away from the edge. For the linear case, n
⫽1, Eq. 共48兲 gives the square-root singularity J(x)
4012
ALEX GUREVICH AND MARK FRIESEN
FIG. 6. Nonlinear current flow around a semi-infinite cut.
Dashed circle shows a contour of constant electric field. For n
→⬁, all circular contours of constant E touch the end of the cut.
PRB 62
FIG. 8. Nonlinear current flow around a corner. For nⰇ1, current streamlines in the upper right quadrant are nearly circular, and
centered in the vertex.
⫽␴E(x)⬀1/兩 x 兩 1/2, both in J(x) and E(x) at 兩 x 兩 →0.24,32 For
nⰇ1, the nonlinearity of J(E) in superconductors enhances
the singularity in E(x)⬀1/兩 x 兩 , while strongly suppressing the
singularity in J(x)⬀1/兩 x 兩 1/n . For the semiconductor-type
nonlinearity, nⰆ1, the situation is the opposite: the singularity in E(x) is suppressed, but enhanced in J(x).
The second example is the rectangular corner shown in
Figs. 7 and 8. There are two different cases of current flow
inside and outside the corner, which correspond to q⫽q ⫹
2
⬎0 and q⫽q ⫺
2 ⬍0 in Eq. 共42兲, respectively. Excluding E
from Eqs. 共42兲 and Eq. 共44兲, we obtain the current streamlines x⫽Re z( ␺ , ␪ ) and y⫽ Im z( ␺ , ␪ ) in the form22

␺
z⫽D
sin 2 ␪
⫹
FIG. 7. Current flow near the corner of a rectangular sample for
a superconductor (n⫽50) 共a兲 and a normal metal 共b兲. The dashed
straight lines in 共a兲 show boundaries of a diverging current domain
wall, defined as a region where 兩 ␪ ⫺ ␲ /4兩 ⬍0.3.
⫹
1⫺1/nq 2
i␪

2 sin 2 ␪ 兲 e , 共49兲
⫹
where D⫽C 1/nq 2 E 1/n
0 /J 0 (nq 2 ⫺1). Each streamline corresponds to a contour of constant ␺ . The evolution of the current distribution with n is shown in Fig. 7. For n⫽1, we have
q⫹
2 ⫽2, thus Eq. 共49兲 gives smooth hyperbolic streamlines,
␺ ⬀xy.24,32 By contrast, the highly nonlinear case nⰇ1 exhibits sharp changes of the current flow direction near the
diagonal somewhat reminiscent of, yet different from the
piece-wise current distribution of the Bean model 共see below兲.
Current flow past the corner in Fig. 8 exhibits quite different characteristics which manifest themselves in the distribution of local orientations, ␪ (x,y). For nⰇ1 Eq. 共43兲
2
gives nq ⫺
k ⬇⫺(n⫹k ⫺1), thus Eq. 共45兲 simplifies to x/y
⫽⫺tan ␪ . The relation x/y⫽⫺tan ␪ describes circular current streamlines centered in the vertex and is valid everywhere, except for narrow regions of angles, ␦ ␪ ⯝n ⫺1/2, near
␪ ⫽0 and ␪ ⫽ ␲ ⫺ ␣ , which correspond to currents flowing
almost parallel to the sample surface. Therefore current flow
around the semi-infinite corner described by exact Eq. 共45兲
exhibits no trace of singular d lines characteristic of the case
shown in Fig. 7共a兲.
The solutions of this subsection contain a scaling constant
C, which remains undetermined for semi-infinite samples. If
the corner is a part of a defect in a finite sample, say, a
PRB 62
NONLINEAR TRANSPORT CURRENT FLOW IN . . .
4013
surface notch or a step in a film, the above solutions describe
current flow only near the corner. The constant C is determined by current distribution far away from the defect and
thus depends on the sample geometry and the boundary conditions 共see below兲. Here we just note that the particular
value of C does not affect the shape of the current stream
lines described by the function ␪ (x,y). This fact enables us
to investigate universal features of the current domain walls,
based on the exact, yet simple solutions 共42兲–共45兲, regardless of the particular geometry of the whole sample.
B. Structure of the current domain wall
The principal question is how the singular d line emerges
in a smooth current distribution as n→⬁. For the Bean
model, the d line manifests itself in a step-wise change of the
current orientation, ␪ (x,y)⫽ ␲ 关 sgn(x⫺y)⫺1 兴 /4, as seen in
Fig. 4共a兲. Although such a step-wise current configuration
satisfies the critical state assumption, J⫽J c , and the continuity of the normal component of J, it has a jump of tangential component J 储 along the d line. Thus this model distribution of J(x,y) cannot exist in steady state, if any electric
field caused by current flow is taken into account. Indeed, a
jump in J 储 on the d line would result in a discontinuity of the
tangential component of E, which violates ⵜ⫻E⫽0.
For finite nⰇ1 this discontinuity is smoothed out, and the
d line turns into a current domain wall of finite thickness
between regions with different orientations of current flow,
as follows from extensive numerical simulations performed
by Brandt.17 Here we address the following questions, which
are rather difficult to resolve through numerical simulations:

which is determined by the nonlinearity of J(E) regardless
of the sample geometry? 共ii兲 Is there an analytic crossover
from large, but finite n to the Bean model behavior at n
→⬁? 共iii兲 Is the d line of the Bean model a true steady state
in the limit n→⬁? 共iv兲 Is there any singularity in current
domain wall in the limit n→⬁?
The exact hodograph solutions show that only the last
proposition is true, while the very existence of the d line
depends on the geometry of current flow. For example, the
Bean model predicts the d lines for current flow both inside
and outside a corner, depending on the magnetic prehistory.
The results of the previous subsection indicate that, although
some sort of singularity on the diagonal remains for the inside flow in Fig. 7共a兲, the outside flow in Fig. 8 always
exhibits nonsingular circular streamlines. The latter solution
also satisfies the Bean model. Therefore we see that even
exponentially weak electric field in the critical state (nⰇ1)
drives the step-wise current distribution in Fig. 4共a兲 into the
nonsingular one in Fig. 7共a兲, corresponding to the true steady
state.
We now consider the structure of the current domain wall
in Fig. 7共a兲 in more detail by analyzing the behavior of the
function ␪ (x,y) near the diagonal, where x⬇y, ␪ ⫽⫺ ␲ /4
2
2 2
⫹ ␦ , and ␦ Ⰶ1. If nⰇ1, we have nq ⫹
k ⬇k ⫺k (k ⫺1)/n, so
Eq. 共45兲 for ␦ Ⰶ1, simplifies to

3
x⫺y
⫽2 ␦ ⫹ ␦ 2 .
x
n

FIG. 9. Structure of the current domain wall for different n
values. The dashed line shows the step-wise dependence ␦ (x,y) of
the Bean model.
From Eq. 共50兲 it follows that there is no ‘‘intrinsic’’ width of
the current domain wall, since ␦ (x,y) is a power-law function of x and y near the diagonal. If we define the domain
wall as a region, in which ␦ ⬍ ␦ 0 , then Eq. 共50兲 gives its
width, d(l 储 , ␦ 0 ), as a function of the conditional criterion ␦ 0
and the distance l 储 ⫽(x⫹y)/2 from the vertex along the diagonal. We thus obtain that the so-defined width of the current domain wall, d⫽ ␦ 0 (3/n⫹ ␦ 20 )l 储 linearly increases with
l 储 and remains finite even in the limit n→⬁. The dependence
of ␪ (l 储 ,l⬜ ) on the coordinate l⬜ ⫽(x⫺y)/2 across the d line
at a fixed distance l 储 from the vertex is shown in Fig. 9. For
finite n, we obtain that ␦ ⫽nl⬜ /3l 储 is linear when l⬜
Ⰶl 储 (3/n) 3/2 and acquires the universal dependence ␦
⫽(l⬜ /l 储 ) 1/3 when l⬜ Ⰷl 储 (3/n) 3/2 . Therefore the exact theory
predicts continuous broadening of the d line with l 储 , as observed in magneto-optical experiments.7
In the limit n→⬁, we have ␦ ⫽(l⬜ /l 储 ) 1/3 for all l⬜ , thus
the function ␪ (l⬜ ) remains continuous at l⬜ ⫽0, but the derivative ⳵ ␪ / ⳵ l⬜ ⬀l⬜⫺2/3 diverges, in stark contrast to the jump
in ␪ (x,y) for the Bean model. Such a ‘‘soft’’ singularity in
␪ (x,y) is rather difficult to reveal in numerical simulations
of nonlinear Maxwell’s equations in the coordinate space.
Therefore, for n→⬁, some kind of singular d lines do appear, but the behavior of ␪ (l 储 ,l⬜ ) turns out to be quite different from the Bean model 共see Fig. 9兲. This difference is
due to the fact that the hodograph solutions satisfy the condition ⵜ⫻E⫽0, even for n→⬁.
V. PLANAR DEFECT IN AN INFINITE
SUPERCONDUCTOR
Now we consider a more complicated problem of current
flow past a thin nonconducting planar defect of length 2a in
an infinite media 共Fig. 10兲. This case models the strongest
current-limiting defects in HTS’s, such as high-angle grain
ALEX GUREVICH AND MARK FRIESEN
4014
PRB 62
weak. In this case it is convenient to write Eq. 共26兲 in polar
coordinates (r, ␹ ), with the origin at the end of the cut, ␩
⫽0, ␪ ⫽ ␲ /2:
⳵ rr h⫹r ⫺1 ⳵ r h⫹r ⫺2 ⳵ ␹␹ h⫺ ␤ 2 h⫽0,

where ␩ ⫽r cos ␹, ␪ ⫽ ␲ /2⫹r sin ␹, and ␤ is given by Eq.

If ␲ ␤ →⬁, the function h(r, ␹ ) describes a vortex at the
end of the cut in an infinite media. In this case, an exact
vortex solution of Eq. 共53兲 is
h⫽ 冑2h 0
FIG. 10. Mapping of the current flow around a thin nonconducting strip in the xy plane 共inset兲 onto the hodograph plane ␩ ␪ .
boundaries, or microcracks. To capture the general features
of ␺ ( ␩ , ␪ ), we first consider the complex potential w(z) for
the same geometry in the case of Ohmic conductors,24
w⫽iE 0 冑z 2 ⫺a 2 .

Expressing w via the complex electric field, E exp(⫺ı␪)⫽
⫺dw/dz 共see Appendix A兲, we obtain
w⫽⫺
aE 0

,

where ␩ ⫽ln(E/E0). As follows from Eq. 共52兲, the stream
function ␺ ⫽Im(w) has a singularity at ␩ ⫽0, ␪ ⫽ ␲ /2 and
decays exponentially away from this point, on the scale ␩
⬃1, ␪ ⫺ ␲ /2⬃1.
The boundary conditions for ␺ ( ␩ , ␪ ) in the hodograph
plane follow from the symmetry properties of the current
flow around the defect 共Fig. 10兲. First, we notice that the
zero x component of J on the central line 共perpendicular to
the defect兲 requires the boundary condition ␺ ( ␩ , ␲ /2)⫽0.
Along the ray x⫽0,⫺⬁⬍y⬍0, the electric field varies from
its value at infinity, E⫽E 0 , to zero at the stagnation point,
z⫽0, in the center of the planar defect. Furthermore, the zero
normal component of J on the defect surface also requires
␺ ( ␩ ,0)⫽ ␺ ( ␩ , ␲ )⫽0, with E changing from 0 at z⫽0 to
infinity at the edges (z⫽⫾a). In the hodograph plane ( ␩ , ␪ ),
these boundary conditions give ␺ ⫽0 along two vertical lines
at ␪ ⫽0 and ␪ ⫽ ␲ and along the half-infinite line ⫺⬁⬍ ␩
⬍0 at ␪ ⫽ ␲ /2 共Fig. 10兲. Along the ray, ␩ ⬎0, ␪ ⫽ ␲ /2, we
have ⳵ ␪ ␺ ⫽0. Therefore the problem reduces to the solution
of the London Eq. 共26兲 that describes a ‘‘vortex’’ at the end
of the half-infinite cut, in the center of a superconducting
film of thickness ␲ . The nonlinearity results in effective
‘‘screening’’ in Eq. 共26兲, making h( ␩ , ␪ ) more localized
near the end of the cut in Fig. 10. For nⰇ1, h( ␩ , ␪ ) decays
exponentially over the scale ⬃1/␤ Ⰶ1, so the influence of
the boundary conditions on h( ␩ , ␪ ) at ␪ ⫽0, ␲ becomes very
e ⫺␤r
␹
cos .
2

Solutions with higher order harmonics ⬀ cos m␹/2, give unphysical distributions J(x,y), which we do not consider here.
To satisfy the boundary condition ␺ ⫽0 at ␪ ⫽0,␲ , for
finite ␤ , we use the method of images, by presenting ␺ as a
superposition of the fields of alternating vortices and antivortices at ␩ ⫽0, ␪ ⫽ ␪ m ⫽ ␲ (m⫹1/2), where m⫽0,⫾1, . . . .
This yields
␺ ⫽h 0 兺 共 ⫺1 兲 m

rm
m
e ⫺ ␤ (r m ⫹ ␩ ) ,

where r m ⫽ 冑␩ 2 ⫹( ␪ ⫺ ␪ m ) 2 , and h 0 is a scaling constant,
which will be obtained below. For nⰇ1, the sum in Eq. 共55兲
converges very rapidly, since exp(⫺␤␲)Ⰶ1, thus we can retain only nearest neighbors (m⫽0,⫾1).
Now we come back to the general Eq. 共31兲, in which
B 1,2⫽ ␾ m ⫽0 by symmetry, and C m are just the Fourier coefficients of the function ␺ (E 0 , ␪ ):
C m⫽
4
␲

␲ /2
0
␺ 共 E 0 , ␪ 兲 sin m ␪ d ␪ .

For nⰇ1, ␺ (E 0 , ␪ ) is localized around ␪ ⫽ ␲ /2, so we extend
the upper limit in Eq. 共56兲 to infinity and retain
only the term with m⫽0 in Eq. 共55兲. Then ␺ (E 0 , ␪ )
⫽h 0 exp(⫺␤兩␪⫺␲/2兩 )/ 冑兩 ␪ ⫺ ␲ /2兩 , and Eq. 共56兲 gives C m
⫽(4h 0 / 冑␲ )Im关 exp(im␲/2)/ 冑␤ ⫺im 兴 , whence
C 2k ⫽h 0
C 2k⫺1 ⫽h 0
2 3/2共 ⫺1 兲 k

2 3/2共 ⫺1 兲 k

where ␣ m ⫽ 冑␤ 2 ⫹m 2 , and k is any integer. To satisfy the
boundary condition ␺ ( ␩ , ␲ /2)⫽0 for E⬍E 0 , we take m
⫽2k in Eq. 共31兲. For E⬎E 0 , we have ⳵ ␺ / ⳵ ␪ ⫽0 at ␪
⫽ ␲ /2, hence m⫽2k⫺1. As a result, Eq. 共31兲 can be presented in the form
⬁
␺ ⫽ 兺 C 2k
k⫽1

E
E0
⫹
q 2k
sin 2k ␪ ,
E⬍E 0 ,

NONLINEAR TRANSPORT CURRENT FLOW IN . . .
PRB 62
⬁
␺ ⫽ 兺 C 2k⫺1
k⫽1

E0
E
4015
⫺

sin共 2k⫺1 兲 ␪ ,
E⬎E 0 .

To transform ␺ (E, ␪ ) back onto the xy plane, we substitute Eqs. 共59兲 and 共60兲 into Eq. 共35兲. Since E⫽0 at z⫽0, we
obtain z(E, ␪ ) in the region of E⬍E 0 , integrating Eqs. 共35兲
over E from 0 to E:
z⫽⫺
⬁
e i␪
J0

k⫽1
C 2k

E
⫹
nq 2k ⫺1 E 0
⫹
q 2k ⫺1/n
⫹
⫻ 关 2k cos 2k ␪ ⫺inq 2k
sin 2k ␪ 兴 ,
E⬍E 0 .

In the region where E⬎E 0 , we use the fact that E⫽⬁ at z
⫽a. Substituting Eq. 共60兲 into Eq. 共35兲 and integrating over
E from ⬁ to E, we obtain for E⬎E 0 :
e i␪
z⫽a⫹
J0
⬁

k⫽1

C 2k⫺1
E0
n 兩 q 2k⫺1 兩 ⫹1 E
⫺

⫻ 关共 2k⫺1 兲 cos共 2k⫺1 兲 ␪ ⫹in 兩 q 2k⫺1 兩 sin共 2k⫺1 兲 ␪ 兴 .

The constant h 0 calculated in Appendix B is determined by
the self-consistency condition z(⫹0,0)⫽z(⫺0,0), which
gives for nⰇ1
h 0 ⫽J 0 an 3/4/ 冑2 ␲ .

The current flow described by Eqs. 共59兲–共63兲 is very different from that of Ohmic conductors 共Fig. 11兲.35 The most
visible manifestation of nonlinearity is the long-range disturbance of current streamlines on the scales much larger than
the defect size, 2a. If n→⬁, the magnitude of J(x,y)⫽J c
remains approximately constant everywhere, but a region
near the central line, x⫽0. In addition, the vector J changes
the direction at diverging current domain walls, reminiscent
of the d lines for magnetization current flow past a cylindrical hole in the Bean model 共Fig. 4兲. For finite n, the width of
the current domain walls increases as the distance from the
strip increases, providing the decay of current perturbations
on the scale L⬜ Ⰷa.
Spatial scales of nonlinear current flow around the strip
can be obtained by considering electric-field distributions
along two symmetry lines: in the plane of the defect (y
⫽0, x⬎a, ␪ ⫽ ␲ /2), and along the central line (x⫽0, y
⬍0, ␪ ⫽ ␲ /2). In the first case, substituting Eq. 共55兲 into Eq.

E
E0
x⫺a
erfc ln1/2
⫽
⫺
1/2
L⬜
n
E
0
E ln 共 E/E 0 兲
L⬜ ⫽ 冑2h 0 n 1/4/J 0 ⫽an/ 冑␲ .
,

For nⰇ1, the last term in Eq. 共64兲 关proportional to the error
function erfc(x)兴 can be neglected. As shown in Appendix C,
Eq. 共64兲 is valid everywhere, except the very narrow vicinity
of the defect edge x⫺a⬍a 冑n exp(⫺n/8), where E→⬁. In
FIG. 11. Current flow around a planar defect 共only one quadrant
is shown兲. 共a兲 corresponds to a superconductor described by Eqs.

current flow around the planar defect in Ohmic conductors, where
perturbations of J(x,y) and E(x,y) decay on the length ⬃a.
this region we can retain only one term, k⫽1, with the
⫺

smallest exponent 兩 q 2k⫺1
For nⰇ1, this yields
E 0x ⫾
E 共 x,0兲 ⬇
,

J 共 x,0兲 ⫽J 0

x⫾

1/n
,

where x ⫹ ⫽ 兩 C 1 兩 /J 0 ⫽4a 冑n/ ␲ for x⬎a, and x ⫺ ⫽ 兩 C 1 兩 /nJ 0
⫽4a/ ␲ 冑n for x⬍a. Thus the nonlinearity of E(J) strongly
ALEX GUREVICH AND MARK FRIESEN
4016
FIG. 12. Distributions of E y (x) in the plane of the defect (y
⫽0), described by Eq. 共64兲 for nⰇ1, and by Eq. 共67兲 for n⫽1. For
x⫺aⰆa, the curves have the slopes ⫺1 for nⰇ1 and ⫺1/2 for n
⫽1, because near the edge of the defect, E⬀ 兩 x⫺a 兩 ⫺1 and E
⬀ 兩 x⫺a 兩 ⫺1/2 for superconductors and normal metals, respectively.
The kink in ln(E/E0⫺1) at E⬃E 0 corresponds to a crossover to the
large-x asymptotics: E⫺E 0 ⬃nE 0 (a/x) 2 at x⬃L⬜ .
suppresses the singularity in J(x), while enhancing the singularity in E(x) at x⫽a, as compared to the Ohmic case, for
which24
E 共 x,0兲 ⫽
E 0x

,

n⫽1, x⬎a.
Several important results follow from Eqs. 共64兲 and 共65兲,
as shown in Fig. 12. First, the nonlinearity of E(J) considerably enhances a characteristic magnitude E m of the electric
field. Since E⬃anE 0 /(x⫺a) over a wide region, x⬍L⬜ ,
near defect, we have
E m ⬃nE 0 ⰇE 0 ,
L⬜ ⬃naⰇa.
PRB 62
FIG. 13. Distribution of E(y) along the central line, x⫽0, described by Eq. 共69兲 for nⰇ1 and by Eq. 共70兲 for n⫽1. The length
L 储 of a region of suppressed E(y) scales as a 冑n.
E 共 0,y 兲 ⫽
E 0兩 y 兩

,
n⫽1.

For n⫽1, both E(0,y)⬀ 兩 y 兩 and J(0,y)⬀ 兩 y 兩 decrease linearly
near the stagnation point y⫽0, restoring their background
values E 0 and J 0 on the scale y⯝a. By contrast, for nⰇ1,
we observe a long-range depression of E(0,y) on a scale
L 储 Ⰷa, and a cusp in J(0,y) 共Figs. 13 and 14兲.
The behavior of E(0,y) and J(0,y) at yⰆa can be obtained by taking the term with the minimum exponent with
k⫽1 in Eq. 共69兲, which yields for nⰇ1

Equation 共64兲 predicts a rather slow hyperbolic dependence
of E(x,0) with no definite length scales, so the estimate 共68兲
only gives a characteristic mean value of E(x,0) in the region x⬃L⬜ , where E m ⰇE 0 . Here L⬜ quantifies a distance
from the defect where E(x,0)⯝anE 0 /x becomes of the order of the background electric field E 0 . For larger distances,
x⬎L⬜ , the parabolic dependence E(x,0)⬀1/(x⫺a) gradually turns into a more rapid decay, E(x,0)⫺E 0
⬃(an/x) 2 E 0 for xⰇL⬜ 共Fig. 12兲.
Distributions of E(0,y) and J(0,y) along the central line
(x⫽0) are also strongly affected by the nonlinearity 共Fig.
13兲. To calculate E(y), we set ␪ ⫽ ␲ /2 in Eq. 共61兲 and obtain
⬁

k⫽1
k 冑␣ 2k ⫺ ␤

E
␣ 2k 共 ␣ 2k ⫺ ␤ ⫺n ⫺1/2 兲 E 0
␣ 2k ⫺ ␤ / 冑n⫺1/n
,

where y 0 ⫽2 5/2h 0 / 冑␲ nJ 0 ⫽4an 1/4/ ␲ . The dependence
E(0,y) for nⰇ1 is rather different from that for Ohmic conductors,
FIG. 14. Distribution of J(y) along the central line, x⫽0, described by Eq. 共86兲 for n→⬁ and by Eq. 共82兲 for n⫽1.
NONLINEAR TRANSPORT CURRENT FLOW IN . . .
PRB 62
4017
A. Local flux flow near sharp edges
The above solutions, obtained for the power-law E(J),
exhibit singularities of the electric field E(x)⬀1/(x⫺a) near
the edges of planar defects. Such a strong enhancement of
E(x) indicates that local flux flow can be induced near the
edges, even though the E 0 away from the defect is much
smaller than the crossover electric field E c between flux flow
and flux creep regimes. Description of the current flow near
the edges requires accounting for the full nonlinear dependence E(J).
First we consider current flow near a half infinite cut, for
which the solution of the hodograph Eq. 共21兲 should satisfy
the boundary conditions ␺ (E,0)⫽ ␺ (E, ␲ )⫽0. This solution
of Eq. 共21兲 has the following simple form, valid for any
E(J):
␺⫽
FIG. 15. Surface plot of E(x,y) distribution around a planar
defect for n⫽20. Shown also are the contours of constant E on the
xy plane.
E 共 0,y 兲 ⬀ 兩 y 兩 n/3.

For nⰇ1, the electric field becomes exponentially small in a
wide ‘‘shadow’’ region y⬃a 冑n near the defect. For nⰇ1,
the length scale of variation of E(0,y) can be obtained by
replacing the summation in Eq. 共69兲 by integration, which
results in 共see Appendix C兲

E 共 0,y 兲 ⫽E 0 exp ⫺
L 2储
y
2
,
L 储 ⫽a

n
.
␲

This formula gives a good approximation of the exact Eq.

Eq. 共72兲 that a characteristic length scale L 储 of E(0,y) becomes much greater than a for nⰇ1. For yⰇL 储 , the electric
field E(0,y) approaches E 0 as E(0,y)⫺E 0 ⯝n(a/y) 2 E 0 . Notice that the ratio L⬜ /L 储 ⫽ 冑nⰇ1 is in agreement with the
general result 共16兲. Although Eq. 共72兲 well describes E(y)
for y⬎L 储 , it becomes invalid for y⬍L 储 , where the exponential decrease of E(y) given by Eq. 共72兲 is very different from
the exact result E⬀ 兩 y 兩 n/3. Most clearly, this difference manifests itself in current density distributions for y⬍L 储 : instead
of the exponential decrease J(y)⬀exp(⫺a2/␲y2) given by
Eq. 共72兲, the exact J(y) exhibits a characteristic cusp of the
form J(y)⬀ 兩 y 兩 1/3 共see Fig. 14兲.
Shown in Fig. 15 is the spatial distribution of the modulus
E(x,y), which reveals characteristic scales of the electricfield variation in all directions. The surface plot of E(x,y)
also gives a good approximation for the spatial distribution
of local dissipation Q⫽JE near defect for nⰇ1. In this case
variations of J(x,y) are week, thus Q(x,y)⫽J 0 E(x,y) to a
very good accuracy. The strong, long-range disturbance of
E(x,y) near the defect results in a significant excess dissipation, as will be shown below.

where the constant A will be obtained below. To calculate
z(E, ␪ ), we substitute Eq. 共73兲 into Eq. 共34兲 and integrate
over ␪ , which yields
z⫽⫺
J 共 0,y 兲 ⬀ 兩 y 兩 1/3,
A
sin ␪ ,
E
A 2i ␪
e ⫹ f 共 E 兲.
2EJ

Here f (E) is a real function of E 关the imaginary part vanishes because of the boundary condition y(E,0)⫽y(E, ␲ )
⫽0兴. The equation for f can be obtained by substituting Eqs.

⳵E f ⫽

1
A ␴
⫺
.
2 J 2 E JE 2

The boundary condition for f (E) follows from the fact that
the electric field E(x,y) becomes infinite at the end of the
cut (x⫽y⫽0), as shown in Fig. 6. Then Eq. 共74兲 gives
f (⬁)⫽0, and integration of Eq. 共75兲 yields
f 共 E 兲 ⫽A

⬁ dE ⬘
E
⫺
JE ⬘ 2

1
.
2JE

Equations 共73兲, 共74兲, and 共76兲 give a solution of the nonlinear Maxwell equations, which describe current flow around
the half infinite cut for arbitrary J(E). This solution also
describes approximately the current flow near the edge of a
cut of finite length 2a, where the scaling constant A is determined by the current flow on the length of order a away
from the edges.
To calculate A we need to match Eq. 共73兲 with the solution of the previous section, which describes current flow
around a cut of length 2a, for the power law J(E). To do so
we note that for EⰆE c , the power-law approximation is
valid everywhere around the cut, except small regions near
the ends. Here EⰇE 0 , so the main contribution to ␺ comes
from the term with k⫽1 and minimum 兩 q ⫺
k 兩 in Eq. 共60兲. This
yields the same universal dependence ␺ (E, ␪ )
⫽C 1 (E 0 /E)sin ␪ as Eq. 共73兲, whence A⫽C 1 E 0 . Using Eqs.

4018
ALEX GUREVICH AND MARK FRIESEN
A⫽
2 5/2h 0 n 3/4E 0

⫽
4 冑n
aJ 0 E 0 .
␲

Separating real and imaginary parts of Eq. 共74兲, we get
x⫺ f 共 E 兲 ⫽⫺
y⫽⫺
A
cos 2 ␪ ,
2JE
L⬜ ⬃anE 0 /E c ,

Thus the contours of constant E are circles of radius A/2JE
centered at x⫽ f (E), y⫽0 共Fig. 6兲. Equation 共78兲 and 共79兲
describe the intermediate asymptotics of the current distribution in a small region of radius RⰆa near the edge 共see
below兲. Away from the edge, Eqs. 共78兲 and 共79兲 merge with
the solution of the previous section, which describes the current flow around the cut and provides the correct asymptotics
E→E 0 at infinity.
We can further simplify Eq. 共76兲, using the fact that J(E)
in superconductors varies rather weakly, even for significant

Since the main contribution to the integral in Eq. 共76兲 comes
from E ⬘ ⯝E, we can therefore take the slowly varying function J(E ⬘ )⬇J(E) out of the integral and obtain
f ⫽A/2JE.

2a 冑n E 0
A
⫽
.
R⫽
2J c E c
␲
Ec

Excluding ␪ from Eqs. 共78兲–共80兲, we obtain the electric-field
distribution near the edge:
␲ 共 x 2 ⫹y 2 兲
,
L 储 ⬃a 冑nE 0 /E c .

The condition that the flux flow region is much smaller than
a now requires E 0 ⰆE c /n.
The hodograph method enables us to trace the evolution
of current flow with n and see what happens in the critical
state limit, n→⬁. Because of the ambiguity of the Bean
model discussed in the Introduction, current flow in the true
critical state should be first calculated for large, but finite n
values and only then the limit n→⬁ is to be taken. We
consider this rather nontrivial limit in detail for current flow
past a planar defect, assuming that J 0 ⫽J c at infinity. As was
shown before, the solution for J(x,y) describes two regions
of current flow, corresponding to J⬍J c and J⬎J c . The solutions for J⬍J c can be obtained from Eqs. 共61兲 straightforwardly, by taking the limit n→⬁. However, the solutions
with J⬎J c should be handled with care, since in the Bean
model, current densities J⫽J c ⫹0 correspond to infinite E.
For J⬍J c , and n→⬁, the stream function ␺ described by
Eq. 共61兲 can be presented in the following form independent
of n:

To calculate corrections to f (E) due to flux flow, we assume
that J(E)⫽J c ⫹ ␴ f E for E⬎E c , where ␴ f is the flux flow
conductivity. Then the integration of Eq. 共76兲 gives f
⬵A/2J c E⫹A ␴ f /2J 2c , if ␴ f E/J c Ⰶ1.
The radius R of the circular flux flow region near the edge

and 共79兲 and substituting there Eqs. 共77兲 and 共80兲:
E 共 x,y 兲 ⫽
that as E 0 increases, the size of the flux flow region along the
x axis, L⬜ , turns out to be much larger than its size, L 储 ,
along the y axis:
B. Critical state limit, n\ⴥ
A
sin 2 ␪ .
2JE
4a 冑nxE 0
PRB 62
x⬎0.

The above matching of two solutions near the edge and
around the strip is justified, if the radius of the flux flow
region R is small compared to the length of the strip 2a.
From Eq. 共81兲 we find that RⰆa if E 0 ⰆE c / 冑n. This condition indicates that because of the enhancement of the electric
field near the edges, the local flux flow occurs when the bulk
E 0 is much smaller than the crossover field E c . However,
there is a much stronger applicability condition of the above
description, based on the one-term approximation of the sum
in Eq. 共62兲. As shown in Appendix C, the terms with k⬎1 in
Eq. 共62兲 can be neglected, if E 0 ⰆE f ⬃E c exp(⫺n/8). For
E 0 ⰇE f , the flux flow region near the edge becomes noncircular, being essentially stretched out along the x axis 关Fig.
11共a兲兴. An analysis of this case given in Appendix C, shows
8aJ c
␺⫽
␲
⬁

J

Jc
k
k⫽1
4k 2

⬁
z⫽⫺
sin 2k ␪ ,
16a i ␪

e
␲
Jc
k⫽1 4k 2 ⫺1

4k 2 ⫺1
⫻ 共 cos 2k ␪ ⫺2ik sin 2k ␪ 兲 .

The sums in Eqs. 共84兲 and 共85兲 can be expressed in terms of
elliptical theta functions.37 The asymptotics of J(x,y) considerably simplify far away from the defect, ( 兩 z 兩 Ⰷa), as
shown in Appendix D.
From Eqs. 共85兲, we obtain the current distribution J(y)
along the central line x⫽0, ␪ ⫽ ␲ /2,
16a

␲
⬁

k⫽1
k2

J
2
4k ⫺1 J c
4k 2 ⫺1
,

which is shown in Fig. 14. Near the stagnation point, y→0,
the function J(y)⯝J c (3 ␲ y/16a) 1/3 exhibits a cusp. Notice
that J(y) restores the bulk value J c on the length ⬃a, unlike
the electric field E(y), which varies on the scale ⬃a 冑n.
The limit n→⬁ cannot be directly taken in the region J
⬎J c , since the sum in Eq. 共62兲 diverges. So we first consider
the well-behaved case of large, but finite, n and calculate the
boundary between the regions of current flow with E⬎E 0
and E⬍E 0 in the real space 关see Fig. 16共a兲兴. As shown in
Appendix D, the boundary is given by the curve y(x), which
for nⰇ1 is described parametrically as follows:
x⫺a⫽h 0
e ⫺ ␤␥

,

NONLINEAR TRANSPORT CURRENT FLOW IN . . .
PRB 62
4019
the singular line V 0 ⬃a 冑nE c (J 0 /J c ) n , vanishes. Thus we
may ignore the region E⬎E 0 , and Eqs. 共84兲 and 共85兲 give a
complete description of the current distribution in the true
critical state, E⫽0. Shown in Fig. 16共b兲 are the current
streamlines given by Eqs. 共84兲, which are practically indistinguishable from those for large but finite n values in Figs.
11共a兲 and 16共a兲. However, the dc electric field distribution
for large but finite n remains very different from the critical
state predictions. Indeed, instead of converging to a straight
line along the x axes, the region of E⬎E 0 in Fig. 16共b兲
significantly extends along the direction of current flow even
for n⫽300, which is much larger than typical values of n
⬃10–50 for superconductors.
In the limit, n→⬁, current flow around the defect has the
singular d lines, which come out of the stagnation points and
extend to infinity as shown in Fig. 16共b兲. Near the stagnation
point the d lines make a 45° angle with the x axis and have
the same structure as for current flow near the corner, described by Eq. 共50兲. For ( 兩 z 兩 Ⰷa), the following simple equation of the d line can be obtained, as shown in Appendix D:

x⫽y 2 /y ⬁ ,
where y ⬁ ⫽8a/ 冑2 ␲ e⬇1.94a. Therefore, far away from the
planar defect, the d lines become parabolic, whereas the current streamlines between the d lines in Fig. 15共b兲 are approximately circular, to the accuracy of slowly varying logarithmic factors 共see Appendix D兲. These results are
qualitatively similar to current flow around the cylindrical
void in the Bean model 共Fig. 4兲. However, unlike Bean’s d
line in Fig. 4, current flow near the d lines described by exact
Eqs. 共85兲 exhibits no discontinuity in the tangential component of J, thus satisfying the condition ⵜ⫻E⫽0, even in the
limit n→⬁.
VI. DISSIPATION NEAR PLANAR DEFECTS
In this section we obtain a general expression for the excess total dissipation Q due to defects:
Q⫽
FIG. 16. Current flow around the planar defect for large 共a兲 and
infinite 共b兲 n values, described by Eqs. 共59兲–共63兲 and Eqs. 共84兲 and

between the regions of current flow with E⬎E 0 and E⬍E 0 . In the
limit n→⬁, this boundary reduces to a ray, y⫽0, shown in 共b兲. The
dashed line in 共b兲 shows the d line, which is well described by the
parabolic function 共89兲 for x⬎2a.

1

⫹ 冑␥ e ⫺ ␤␥ ,

where ␥ ⫽ ␲ /2⫺ ␪ . From Eqs. 共87兲 and 共88兲, we obtain that

→⬁, the whole region of E⬎E 0 reduces to a ray along the x
axis, where the electric field formally diverges. The voltage
across this region, V 0 ⬃E(x)⌬y, is of order E 0 a 冑n, since
E(x)⬃E 0 an/(x⫺a), and ⌬y⬃(x⫺a)/ 冑n. In the limit n
→⬁, we should take J 0 ⫽J c ⫺0, so that the voltage across

dx dy 共 JE⫺J 0 E 0 兲 ,
where the term J 0 E 0 corresponds to a uniform sample without defects. Now we transform from integration over x and y
to the hodograph variables, E and ␪ , and obtain 共see Appendix E兲

2␲
Q⫽
⬁
d
0
0

␴
dE

J ␪
J

Substituting Eq. 共28兲 into Eq. 共91兲 and integrating over ␪
from 0 to 2 ␲ , we present Q in the form
Q⫽ ␲

⬁

␴ m 2 2 dE
f
.
J m J2

Here integration from 0 to 2 ␲ implies that current flow contains all possible orientations of J, as it occurs for a planar
defect in an infinite superconductor.
4020
ALEX GUREVICH AND MARK FRIESEN
We apply these formulas to calculate dissipation power Q,
caused by planar defects. We first consider a simpler case of
a semi-infinite cut in Fig. 6 and calculate the total dissipation
power ⌬Q inside a circular region at the edge where E exceeds a certain electric-field threshold, E c . Substituting Eq.

seen from Fig. 6, the current flow around a semi-infinite,
unlike planar defects of finite length, is represented by only
half of the hodograph plane, 0⬍ ␪ ⬍ ␲ ). Integrating then over
E, as explained in Appendix E, we obtain a simple exact
result,
⌬Q⫽ ␲ A 2 /2J c E c ,

valid for any J-E relation. For instance, if E c is chosen in the
flux creep region, ⌬Q is unaffected by the flux flow portion
of E(J).
Now we calculate Q for a planar defect of length 2a for
the power-law E(J) characteristic. Substituting Eq. 共23兲 into
Eq. 共91兲 and integrating over E, we obtain
⬁

⫺
2
⫹
2
q 2m

C 2m
␲E0
,
⫺
Q⫽

⫺
⫹
2J 0
m⫽1
n 兩 q 2m⫺1

nq 2m
⫺1

where the subscripts ⫹ and ⫺ corresponds to the signs in
front of the square root in Eq. 共32兲. The positive terms, pro2
in Eq. 共94兲, represent an excess dissipaportional to C 2m⫺1
tion due to enhanced electric field around a defect, while the
2
, account for reduced
negative terms, proportional to C 2m
dissipation in the stagnation regions. For Ohmic conductors,
these two opposite contributions exactly cancel each other,
giving Q⫽0 for n⫽1 共see Appendix E兲. For nⰇ1, the spatial distribution of Joule dissipation JE is similar to E(x,y)
shown in Fig. 15. In this case, there appears an excess dissipation (Q⬎0), since the contribution to Q from the electricfield enhancement along the x axis 共on the scale L⬜ ⬃na) is
much greater than the negative contribution of the stagnation
regions 共on the scale L 储 ⬃ 冑na). Substituting Eqs. 共58兲 for
C m , into Eq. 共94兲 and evaluating the sum as explained in
Appendix E, we obtain
Q⫽J 0 E 0 a 2 共 n⫺1 兲 冑n.

For nⰇ1, Eq. 共95兲 is an exact asymptotics of Q(n), which
approximates Eq. 共94兲 to an accuracy better than 1% for n
⬎10 and 6% for 5⬍n⬍10. The physical meaning of Eq.

Q⯝ ␲ L 储 J 0 兰 ⬁a (E⫺E 0 )dx, which is just the excess dissipation
in the region of substantial enhancement of E(r) by the defect. Using Eqs. 共64兲 and 共65兲 for E(x), we obtain
Q⬃ ␲ J 0 E 0 L 储 L⬜ , which gives the correct leading term,
Q⯝E 0 J 0 a 2 n 3/2.
VII. DISCUSSION
The analytical results obtained in this paper reveal essential features of nonlinear 2D current flow, which can affect
the current-carrying capability and macroscopic electrodynamics of superconductors. This influence mostly results
from the fact that planar obstacles cause strong enhancement
and long-range decay of electric-field disturbances. These
PRB 62
effects are important for applications, in particular, ac losses,
critical state stability, and current flow in thin-film superconducting circuits. The use of the hodograph technique enabled
us to address such characteristics of nonlinear current flow,
as orientational current flow domains and the structure of
current domain walls. In addition, we were able to trace the
evolution of current distributions with n and a nonanalytic
crossover to the critical state limit, n→⬁, when singular d
lines emerge.
The fact that a planar obstacle of size a greatly enhances
electric-field disturbances over scales L⬜ ⬃an perpendicular
to current flow or L 储 ⬃a 冑n along current flow results in
long-range interaction between defects, and strong effect of
the sample geometry. Indeed, even a sparse network of planar defects can substantially reduce the effective currentcarrying cross section, if the mean spacing between the defects is smaller than L⬃an. For typical values of n⬃30,
such a nonlinear blockage of transport current by defects can
occur at rather small concentration of obstacles, which occupy only few percent of the geometrical cross section of a
superconductor. This effect can have important implications
for current percolation through arrays of planar defects, such
as grain boundaries in HTS polyscrystals 共Fig. 2兲. It also
contributes to multiple current-limiting mechanisms in HTS
conductors, such as Bi tapes and biaxially textured
YBa2 Cu3 O7 coated conductors.38 For instance, a microcrack,
in a film of thickness d 共Fig. 3兲, can cause a strong local peak
of E(x) in YBCO coated conductor, even for rather small
defects a⬎d/nⰆ1. In turn, such local peaks of voltage and
dissipation change the global current-voltage characteristic
of the whole conductor, similar to the effect of macroscopic
random inhomogeneities.12 A detailed analysis of the significant finite-size effects for current flow in restricted geometries shown in Fig. 3 will be given elsewhere.25
The features of nonlinear current flow discussed above
can be observed by the magneto-optical 共MO兲 technique,
which indeed revealed long-range disturbances of the normal
component of H(x,y) around macroscopic defects in
HTS’s.7,9 For instance, characteristic flamelike shapes of the
magnetic-flux disturbances around defects on MO images are
similar to the contours of constant E shown in Figs. 11 and
15. By measuring the scales L⬜ and L 储 of magnetic-flux
disturbance, one can extract both the n value, n⯝(L⬜ /L 储 ) 2 ,
and the size of the defect, a⬃L⬜ /n, even if the defect is
smaller than the MO resolution 共usually ⯝50–10 ␮ m). Extensive stagnation regions (L 储 ⬃a 冑n) of exponentially small
electric field constitute another feature of nonlinear current
flow around planar defects 关Fig. 11共a兲兴 which could be observed in MO experiments. This nonlinear ‘‘shadow effect’’
manifests itself in the distribution of flux velocities, v⫽ 关 H0
⫻E兴 /H 20 , in a strong magnetic field H 0 when vortices move
along equipotential lines, ␸ (x,y)⫽const. Vortex velocity v
sharply increases in the regions of enhanced electric field
near the edges of the planar defect, which thus becomes a
flow channel for magnetic flux 关see Figs. 11共a兲 and 15兴.
These flux jets are sandwiched between two macroscopic
stagnation regions of nearly motionless flux which result
from the geometry of the current flow and the strong nonlinearity of E(J), but are not due to enhanced flux pinning.
PRB 62
NONLINEAR TRANSPORT CURRENT FLOW IN . . .
The excess dissipation Q caused by defects is another
important feature of the strong nonlinearity of E(J). Superconducting materials, and especially HTS’s, contain many
macroscopic current-limiting defects 共microcracks and highangle grain boundaries兲,6 which contribute significantly to
the overall ac losses and dissipation. As an example, we
consider a sparse array of planar defects of size ⬃a spaced
by lⰇa. Then we obtain from Eq. 共95兲 that the defects result
in the excess dissipation power ⬃n 3/2(a/l) 2 J 0 E 0 per unit
volume, which becomes of the order of the background bulk
dissipation power J 0 E 0 , if l⬍an 3/4. Therefore the overall
dissipation will be dominated by defects, if they occupy a
rather small fraction ⬃n ⫺3/4 of the geometrical cross section
of the sample 共few percent for the typical n values ⬃20–30
for superconductors兲. The excess dissipation due to defects
can also trigger local thermal instabilities in high-J c
superconductors.36 Such instabilities develop mostly in the
regions of enhanced heat generation E⬎E 0 in Figs. 11共a兲
and 15, which dominate the overall Q. Another type of orientational current instabilities can be caused by the high anisotropy of HTS’s,21 when current is forced to flow along the
c axis by microcracks8 or a ‘‘brick-wall’’ structure of inplane tilt grain boundaries.39
ACKNOWLEDGMENTS
Another feature of Ohmic conductors is that the complex
potential w(u) is also an analytic function in the hodograph
plane, u⫽ ␩ ⫺i ␪ , where ␩ ⫽ln(E/E0).
In nonlinear conductors, ␳ depends on E, so neither w(z)
nor w(u) are analytic functions. We consider properties of w
for the power law E(J), for which Eqs. 共20兲 can be written in
the following symmetric form:
⳵ ␩ ␸ ⫽ 共 ␳ 0 / 冑n 兲 e 2 ␤ ␩ ⳵ ␪ ␺ ,

⳵ ␪ ␸ ⫽⫺ 共 ␳ 0 / 冑n 兲 e 2 ␤ ␩ ⳵ ␩ ␺ ,

where ␤ ⫽(n⫺1)/2冑n, ␩ ⫽n ⫺1/2 ln(E/E0), and ␳ 0 ⫽E 0 /J 0 .
Defining new functions, h 1 ⫽ ␸ exp(⫺␤␩) and h 2
⫽( 冑n/ ␳ 0 ) ␺ exp(␤␩), we present Eqs. 共A5兲 and 共A6兲 in the
form
2D current flow in Ohmic conductors is described by the
complex potential
w 共 z 兲 ⫽ ␸ ⫺i ␳ ␺ ,

which is an analytic function of z⫽x⫹iy. The analyticity of
w(z) greatly simplifies the calculation of 2D current distributions, allowing exact solutions for the geometries shown in
Fig. 3 to be obtained using conformal mapping.32 The condition that w(z) is an analytic function can be written in the
form
dw
dz̄
⫽0,

where the bar denotes complex conjugate, and the complex
differentiation of any function f (z)⫽u⫹i v is defined as34

1 ⳵u ⳵v
i ⳵v ⳵u
⫽
⫹
.
⫺
⫹
2
⳵
x
⳵
y
2
⳵x ⳵y
dz̄
df
The fact that d f /dz̄⫽0 for any analytic function f (z) follows from the Cauchy-Riemann conditions, ⳵ x u⫽ ⳵ y v , ⳵ y u
⫽⫺ ⳵ x v . The electric-field distribution, E x ⫹iE y ⫽E exp(i␪),
can be calculated from
Ee
⫺i ␪
dw
⫽⫺
.
dz

⳵ ␪h 1⫹ ⳵ ␩h 1⫽ ␤ h 2 .

␤
⫽⫺ w̄ 0 ,
2
dū
dw 0

which describes generalized analytic functions.33 Therefore
calculations of current flow in nonlinear conductors can be
formulated in terms of generalized analytic functions for the
effective potential w 0 (u) in the hodograph plane, u⫽ ␩
⫺i ␪ . This fact enables one to calculate 2D nonlinear current
flow by constructing an appropriate generalized analytical
function,22 using methods which have been developed in the
literature.33 Expressing w 0 in terms of ␸ and ␺ , we obtain
w 0⫽ ␸ e ⫺␤␩⫺
i␳0

e ␤␩␺ .

For n⫽1, the effective potential w 0 reduces to w.
APPENDIX B: NORMALIZATION CONSTANT
To calculate h 0 , we equate Eqs. 共61兲 and 共62兲 to obtain
the self-consistency condition z(⫹0,0)⫽z(⫺0,0), whence
a⫽⫺

⳵ ␩ h 1 ⫺ ⳵ ␪ h 2 ⫽⫺ ␤ h 1 ,
These equations can be combined into a single complex
equation for the effective complex potential, w 0 ⫽h 1 ⫺ih 2 .
Using complex differentiation 共A3兲 with respect to u⫽ ␩
⫺i ␪ , we obtain the equation for w 0 in the form of a firstorder Carleman equation,
We are grateful to D. C. Larbalestier and A. P. Malozemoff for discussions. This work was supported by the NSF
MRSEC 共Grant No. DMR 9214707兲 and EPRI.
APPENDIX A: ANALYTIC PROPERTIES OF THE
COMPLEX POTENTIAL
4021
1
⬁

J 冑n k⫽1
0

2k
2k⫺1
C 2k ⫹
C 2k⫺1 .
uk
pk

It is convenient to write Eq. 共B1兲 as h 0 ⫽⫺aJ 0 /I, where I is
obtained from Eqs. 共57兲 and 共58兲 in the form
I⫽
2 3/2
⬁

⫹

2m 共 ⫺1 兲 m 冑␣ 2m ⫺ ␤

2

␣ 2m⫺1 共 ␣ 2m⫺1 ⫹ ␤ ⫹1/冑n 兲

.
␣ 2m ⫹ ␤ ⫹
1

4022
ALEX GUREVICH AND MARK FRIESEN
For nⰇ1, this sum is dominated by the first term in the
square brackets, where 1/冑n in ( ␣ 2m ⫹ ␤ ⫹1/冑n) can be neglected. Then I reduces to
I⫽
2 3/2
⬁

2
⫹

␣ 2m

.

The first part of this sum, I 1 , is rapidly converging over m
⬃1, so the slowly varying factor 冑␣ 2m ⫹ ␤ / ␣ 2m can be replaced by its constant value at m⫽1. Then the summation
yields
I 1 ⫽⫺
␲ ⫺2

.
The second part of I is an expression of the form I 2
⬁
⫽ 兺 m⫽1
(⫺1) m F m , where F m , given by the second term in
the square brackets, decreases slowly with m for nⰇ1. To
turn I 2 into a rapidly converging series, we write
⬁
I 2⫽
⬁
⬁
1

m⫽1
d k F 2m
dm
k
, 共B5兲
where F m is nearly constant for m⬍ ␤ , and decreases as
1/冑m for m⬎ ␤ . Therefore each differentiation of F m over m
brings a small factor ⬃1/冑n, so the main contribution to I 2
comes from the term with k⫽1. Since dF m /dm is a slow
function of m, we can replace summation in Eq. 共B5兲 by
integration using the Poisson-Euler formula34 written in the
form

m⫽1
⬁
⬁
f 共0兲 ⳵m f 共0兲
⫺
,
2
12

where f m ⫽0.5dF m /dm. Since F m is a function of m 2 , the
second term in the right-hand side of Eq. 共B6兲 vanishes, and
the last term ⬃ ␤ ⫺5/4Ⰶ1 is negligible. As a result, the sum

I 2 ⫽⫺
2

.
Combining I 1 and I 2 , we obtain Eq. 共63兲, which approximates Eq. 共B1兲 to the accuracy better than 1% for n⬎5.
APPENDIX C: ASYMPTOTICS OF z„E, ␪ …
To sum up Eq. 共69兲 at nⰇ1, we consider the region of
x⬍a 冑n, where EⰆE 0 . The convergence of the sum is then
mostly determined by the factors (E 0 /E) ␭ k , where ␭ k
⫽( ␣ 2k ⫺ ␤ )/ 冑n⫺1/n. In this case the main contribution to
Eq. 共69兲 for nⰇ1 comes from the region k⬍ ␤ , where the
slowly varying factor ␣ 2k can be taken out of the sum at k
⫽1. Then ␣ 2k ⫺ ␤ ⬇2k 2 / ␤ , ␭ k ⬇4k 2 /n, and Eq. 共69兲 reduces
to
y⫽
4a
␲
⬁

k⫽1

E
E0
4k 2 /n
.

PRB 62
For nⰇ1, the sum in Eq. 共C1兲 can be evaluated with the use
of Eq. 共B6兲, giving 关 ␲ n/ln(E/E0)兴1/2/4. As a result, we arrive
at Eq. 共72兲. This approach gives the intermediate asymptotics
of E(0,y) at y⬃L 储 . The behaviors of E(0,y) for y→⬁
should be obtained in a different way, since for E→E 0 , the
sum in Eq. 共69兲 diverges. The main contribution then comes
from kⰇ ␤ , and Eq. 共69兲 becomes
y⫽
⬁
a
1

␲ 冑2n 1/4 k⫽1 冑k

E
E0
2k/ 冑n

.
For nⰇ1, evaluation of this sum with the use of Eq. 共B6兲,
gives y⫽a 冑n/ ␲ ln⫺1/2(E 0 /E). This yields the same
asymptotic behavior of E(0,y)⫺E 0 ⫽E 0 (L 储 /y) 2 as Eq. 共72兲.
To calculate the distribution of E(x,y) near the edges, we
write Eq. 共62兲 in the form
z⫺a⫽
2 3/2h 0 e i ␪

⫻

⬁

k⫽1
2k⫺1

p k ␣ 2k⫺1
E
␴k
cos共 2k⫺1 兲 ␪

⫹i 共 ␣ 2k⫺1 ⫹ ␤ 兲 sin共 2k⫺1 兲 ␪ ,

where ␴ k ⫽ 兩 q 2k⫺1 兩 ⫹1/n. Near the edges, where EⰇE 0 , the
convergence of this sum is determined by the small factor
(E 0 /E) ␴ k ⫽exp关⫺␴k ln(E/E0)兴 at (2k⫺1) 2 ⬍n. There are
two characteristic domains. The first one is very close to the
edge (E→⬁), so that the sum 共C3兲 is dominated by the term
k⫽1, for which the exponent ␴ 1 ⫽1⫹1/n is minimum. In
this case the term with k⫽2 is negligible, that is, exp关⫺(␴2
⫺␴1)ln(E/E0)兴Ⰶ1. For nⰇ1, we get ␴ 2 ⫽1⫹9/n, thus the
sum in Eq. 共C3兲 is determined by only one term with k⫽1, if
(8/n)ln(E/E0)⬎1. This criterion defines the size of the region, r c ⬃a 冑n exp(⫺n/8), at the edge, where the one-term
approximation holds.
Since r c decreases exponentially with n, there is a wide
region near the planar defect where ln(E/E0)Ⰷ1, but the
terms with k⬎1 in Eq. 共C3兲 cannot be neglected. In the large
region r c ⰆxⰆan, where EⰇE 0 , the convergence of the sum

much weaker k dependence of ␣ 2k⫺1 can be neglected. In
this case we can replace ␣ 2k⫺1 ⬇ ␤ and expand ␴ k ⬇1
⫹(2k⫺1) 2 /n. As a result, Eq. 共C3兲 for nⰇ1 reduces to
z⫺a⫽

2 5/2h 0 e i ␪ E 0

I⬘
⫹I ,
n

⬁
I共 ␪,␶ 兲⫽

k⫽1
2

Here ␶ ⫽n ⫺1 ln(E/E0), I ⬘ ⫽ ⳵ ␪ I, and I( ␪ , ␶ ) can be expressed
in terms of elliptical theta-functions.37 Notice that I( ␪ , ␶ )
satisfies the ‘‘diffusion’’ equation
⳵ ␶ I⫽ ⳵ ␪␪ I.

PRB 62
NONLINEAR TRANSPORT CURRENT FLOW IN . . .
Separating real and imaginary parts of Eq. 共C4兲, we express
x( ␪ , ␶ ) and y( ␪ , ␶ ) in terms of I( ␪ , ␶ ):
where ␥ ⫽ ␲ /2⫺ ␪ , and
x⫺a⫽l 关共 I ⬘ /n 兲 cos ␪ ⫺I sin ␪ 兴 ,

␺⫽
y⫽l 关共 I ⬘ /n 兲 sin ␪ ⫹I cos ␪ 兴 ,

where l⫽(4a 冑n/ ␲ )(E 0 /E c ). To calculate I( ␪ , ␶ ), we multiply Eq. 共C5兲 by sin(2m⫺1)␪ and integrate from 0 to ␲ /2:

␲ /2
0
␲ ⫺(2m⫺1) 2 ␶
e
,
4
I cos共 2m⫺1 兲 ␥ d ␥ ⫽

where ␥ ⫽ ␲ /2⫺ ␪ . We consider the wide region of E, where
ln(E/E0)⬎1, but ␶ Ⰶ1. The main contribution to the integral
in Eq. 共C9兲 then comes from ␥ Ⰶ1, so we can extend the
upper integration limit to ⬁ and obtain
I共 ␥,␶ 兲⫽

e
.
4 冑␶

This is a well-known solution of the diffusion Eq. 共C6兲,
which describes the evolution of I( ␥ , ␶ ) in an infinite 1D
media after applying a pulse ⬀ ␦ ( ␥ ) ␦ ( ␶ ).34
Substituting Eq. 共C10兲 into Eqs. 共C7兲 and 共C8兲 and using
the fact that ␥ Ⰶ1, we obtain the distribution E(x,y) in the
following parametric form:
y⫽ 关 1⫹1/2 ln共 E/E 0 兲兴 l ␥ I.
x⫺a⫽lI,

h 0e ⫺␤
g⫽
2

ln1/2共 E c /E 0 兲 1⫹
L⬜ ⫽

1
,
2 ln共 E c /E 0 兲

E0
.

an
1/2

The contour y(x) shown in Fig. 11共a兲 is quite different from
the circular flux flow regions of the k⫽1 approximation.
Here the length L⬜ of the domain with E⬎E c along the x
axis becomes much larger than its size L 储 along the y axis.
Indeed, the maximum of y(x)⫽L 储 occurs at x⫽L⬜ / 冑e. Substituting this into Eq. 共C12兲, we obtain
L 储 ⫽a

2n
1
1⫹
␲e
2 ln共 E c /E 0 兲

E0
.
Ec

To the accuracy of slowly varying logarithmic terms, we
again arrive at the universal relation L⬜ ⬃ 冑nL 储 .
APPENDIX D: CRITICAL STATE LIMIT
To calculate the boundary ( ␩ ⫽0) between the regions
E⬍E 0 and E⬎E 0 , we integrate Eq. 共34兲, written in the form
⳵ ␥ x⫽⫺ 共 cos ␥ ⳵ ␥ ␺ ⫹n ⫺1/2 sin ␥ ⳵ ␩ ␺ 兲 e ⫺ ␩ / 冑n /J 0 , 共D1兲
⳵ ␥ y⫽ 共 sin ␥ ⳵ ␥ ␺ ⫺n ⫺1/2 cos ␥ ⳵ ␩ ␺ 兲 e ⫺ ␩ / 冑n /J 0 ,

After differentiating Eq. 共D3兲 in Eqs. 共D1兲 and 共D2兲, we set
␩ ⫽0. From the form of ␺ for ␤ Ⰷ1, it follows that the main
contribution in Eqs. 共D1兲 and 共D2兲, comes from ␥ Ⰶ1. This
allows us to expand sin␥ and cos␥ in ␥ , retaining only linear
and quadratic terms. Then integration of Eqs. 共D1兲 and 共D2兲
from ␥ to ⬁, with the boundary conditions x(⬁)⫽a,y(⬁)
⫽0, yields
x⫽a⫹
y⫽
h 0 e ⫺ ␤␥
J0

h 0 e ⫺ ␤␥
J 0 冑␥
1

⫺
h 0 冑2 ␲
J 0 n 3/4

erfc冑␤␥ ,
3 冑2 ␲ h 0
⫹ 冑␥ ⫹
4J 0 n 5/4

erfc冑␤␥ . 共D5兲
These formulas determine parametrically the boundary y(x)
of the region of enhanced dissipation (E⬎E 0 ) around the
planar defect. For nⰇ1, the terms proportional to the error
function erfc(x) can be neglected, which gives Eqs. 共87兲 and

Now we calculate J(x,y) far away from the defect. To
sum up Eq. 共85兲, we present it in the form
z⫽⫺be i ␪ 共 I 0 ⫹iI ⬘0 兲 ,
⬁
L⬜
,
x⫺a

Excluding ␥ from Eq. 共C11兲, we obtain contours of equal
E(x,y)⫽E c :

4023
I 0⫽

k⫽1

k ⫺1/4
2
e ⫺(4k
2 ⫺1) ␶

cos 2k ␪ ,

where I ⬘0 ⫽ ⳵ ␪ I 0 , b⫽4a/ ␲ , and ␶ ⫽ln(Jc /J)⬎0. We consider
J(x,y) for 兩 z 兩 Ⰷa, where J→J c , thus ␶ Ⰶ1. In this case I 0
reduces to
⬁
I 0⫽

k⫽1
2
e ⫺4k ␶ cos 2k ␥ ⫹
1
4
⬁
cos 2k ␥
,

k⫽1 k 2 ⫺1/4

where the complimentary angle ␥ (x,y)⫽ ␲ /2⫺ ␪ is small

2
omitted the factor e ⫺4k ␶ , inessential for ␶ Ⰶ1. The first sum
is calculated using Eq. 共B6兲, and the second sum equals 2
⫺ ␲ sin ␥. Hence
I 0⫽
I ⬘0 ⫽

e
⫺ sin ␥ ,
4
4 冑␶

8␶
e ⫺␥
3/2
2 /4␶
⫹
␲
cos ␥ .
4

Combining Eqs. 共D6兲 and 共D10兲, we obtain the following
parametric description of z( ␶ , ␥ ):
x⫽⫺b 共 sin ␥ I 0 ⫺cos ␥ I ⬘0 兲 ,

y⫽⫺b 共 cos ␥ I 0 ⫹sin ␥ I 0⬘ 兲 .

4024
ALEX GUREVICH AND MARK FRIESEN
To reveal the d lines, we calculate the function ␥ (x,y)
from Eqs. 共D11兲 and 共D12兲, expressing ␶ for xⰇa,y⬍0 as
follows:
␶ ⫽⫺
␥ 关 x sin ␥ ⫹y cos ␥ 兴
.
2 关 x cos ␥ ⫺y sin ␥ 兴

␥ 共 1⫹ ␥ ␰ 兲
⫽
exp ⫺
,
2
3
␰⫺␥
␲b

8x 2

which determines ␥ (x,y) as a function of x and ␰ ⫽⫺y/x.
Now we find the position of the d line, on which the spatial
derivatives of ␥ (x,y) diverge. Considering Eq. 共D14兲 as an
explicit expression of the form x⫽x( ␰ , ␥ ), we conclude that
⳵ ␥ x⫽0, that is, the gradient of ␥ along the line y⫽⫺ ␰ x
diverges on the d line. Differentiating Eq. 共D14兲 over ␥ for
␰ ⫽const, we obtain that the condition ⳵ ␥ x⫽0 gives ␥ ⫽ ␰ /2.
Substituting this back into Eq. 共D14兲, we arrive at Eq. 共89兲.
APPENDIX E: DISSIPATION
To transform from integration over dxdy to the
hodograph variables in Eq. 共90兲, we write dxdy⫽Wd ␪ dE,
where the Jacobian, W⫽ ⳵ ␪ x ⳵ E y⫺ ⳵ ␪ y ⳵ E x, is calculated using Eqs. 共34兲 and 共35兲. This yields
W⫽

1
J
2
E共 ⳵ E␺ 兲2⫹

␴

J ␪

The value Q does not change sign for any isotropic J(E)
with a positive differential conductivity, ␴ ⫽ ⳵ J/ ⳵ E. This fact
makes the hodograph transformation a single-valued procedure, that is, a given solution ␺ (E, ␪ ) corresponds uniquely
to physical distributions of E and J in the coordinate space
xy.
To calculate ⌬Q in the flux flow region near the edge of
a half infinite cut, we substitute ␺ ⫽A sin ␪ /E in Eq. 共91兲 and
integrate over ␪ from 0 to ␲ :
⌬Q⫽
␲ 2
A
2

⬁
1⫹
Ec

␴ E dE
.
J JE 2
⬁
Ec
dE
2
J E
⫽
1
⫺
E cJ c

⬁
dE
E c JE 2
.
Q⫽
J0
⫺

1
1⫹
n
⬁
m⫽1

2
␣ 2m⫺1

2
␣ 2m

.

J0
m⫽1

1
1
1
1
⫺
⫹␤ 2
⫹ 2
␣ 2m⫺1 ␣ 2m
␣ 2m⫺1 ␣ 2m

,

where
␣ m ⫽ 冑m 2 ⫹ ␤ 2 .
Expanding
1/␣ 2m⫺1 ⬇1/␣ 2m
⫺0.5⳵ m (1/␣ 2m ) in the first parentheses and using Euler’s
formula 共B6兲, we obtain that the sum of the first term in the
square brackets equals 1/2␣ 0 ⫽1/2␤ . The summation of the
second term in the square brackets yields ␲ /2⫺1/2␤ . Combining these two contributions, we obtain
Q⫽2 ␲ E 0 h 20 /J 0 ⫽a 2 J 0 E 0 n 3/2,

where we used Eq. 共63兲 for h 0 . Equation 共E6兲 gives the leading term in the expansion of Q(n) in nⰇ1. In Eq. 共95兲 we
also took into account the next term of order a 2 J 0 E 0 冑n,
obtained from the best fit of the full dependence Q(n) given
by Eq. 共E4兲. Eq. 共95兲 not only well describes the exact Q(n),
but also provides the correct limit Q⫽0 for n⫽1.
In conclusion, we calculate Q for a planar defect in
Ohmic conductors (n⫽1). It is instructive to do so using Eq.

⫽⫺dw/dz in the form
Ee ⫺i ␪ ⫽⫺i
zE 0

.
Substituting Eq. 共E7兲 into Eq. 共90兲, we obtain
Q
⫽
Q0

2␲
d
0
␳c
0

␳2

⫺1 ␳ d ␳ ,

where Q 0 ⫽ ␴ E 20 a 2 , x⫽a ␳ cos ␣, y⫽a ␳ sin ␣. To avoid the
formally diverging integral in the brackets, we introduce an
auxiliary constant ␳ c Ⰷ1 and obtain after integration over ␳
in the limit ␳ c →⬁:

After substituting Eq. 共E3兲 into Eq. 共E2兲, the integral terms
cancel out and we arrive at Eq. 共93兲.
To calculate Q for a planar defect, we present Eq. 共94兲 in
the form
4E 0 h 20
Q⫽
⬁
4E 0 h 20

Integrating the second term in the brackets by parts, we obtain

For nⰇ1, the terms in the brackets decay rather slowly with
m, so the main contribution to the sum comes from mⰇ1. In
this case we can neglect 1/冑n in the denominators and rewrite Eq. 共E4兲 in the form

Substituting Eq. 共D13兲 into Eqs. 共D11兲 and 共D12兲, and expanding in ␥ Ⰶ1, we obtain the following relation:
PRB 62
Q⫽Q 0

␲
0

⫺cos 2 ␣ ln共 1⫺cos 2 ␣ 兲 ⫺1 兴 d ␣ .

The term proportional to ln ␳c vanishes after integration over
␣ . Integrating the second term in Eq. 共E9兲 by parts, we obtain that it cancels the contribution from the last term in the
integrand, giving Q⫽0. Thus a planar defect in an infinite
Ohmic conductor does not cause any excess overall dissipation. In this case excess dissipation at the edges is exactly
compensated by reduced dissipation in stagnation regions.
PRB 62
1
NONLINEAR TRANSPORT CURRENT FLOW IN . . .
G. Blatter, M.V. Feigelman, V.B. Geshkenbein, A.I. Larkin, and
V.M. Vinokur, Rev. Mod. Phys. 66, 1125 共1994兲.
2
E.H. Brandt, Rep. Prog. Phys. 58, 1465 共1995兲.
3
Y. Yeshurun, A.P. Malozemoff, and A. Shaulov, Rev. Mod. Phys.
68, 911 共1996兲.
4
A. Gurevich and H. Küpfer, Phys. Rev. B 48, 6477 共1993兲; A.
Gurevich, Int. J. Mod. Phys. B 9, 1054 共1995兲; A. Gurevich and
E.H. Brandt, Phys. Rev. Lett. 73, 178 共1994兲; E.H. Brandt, ibid.
76, 4030 共1996兲.
5
C.J. van der Beek, P.H. Kes, M.R. Maley, M.J.V. Menken, and
A.A. Menovsky, Physica C 195, 307 共1992兲; A.A. Zhukov, H.
Küpfer, V.A. Ryabchuk, L.A. Ponomarenko, V.A. Murashov,
and Yu. A. Martynkin, ibid. 219, 99 共1994兲; M. Nideröst, A.
Suter, P. Visani, A.C. Mota, and G. Blatter, Phys. Rev. B 53,
9286 共1996兲.
6
D.C. Larbalestier, Science 274, 736 共1996兲; IEEE Trans. Appl.
Supercond. 7, 90 共1997兲.
7
A.E. Pashitski, A. Gurevich, A.A. Polyanskii, D.C. Larbalestier,
A. Goyal, E.D. Specht, D.M. Kroeger, J.A. DeLuca, and J.E.
Tkaczykl, Science 275, 367 共1997兲; A. Polyanskii, A. Pashitski,
A. Gurevich, J.A. Parrel, M. Polak, D.C. Larbalestier, S.R. Foltyn, and P.N. Arendt, Adv. Supercond. 9, 469 共1997兲.
8
M. Polak, J.A. Parrell, A.A. Polyanskii, A.E. Pashitski, and D.C.
Larbalestier, Appl. Phys. Lett. 70, 1034 共1997兲; X.Y. Cai, A.
Polyanskii, Q. Li, G.N. Riley, and D.C. Larbalestier, Nature

9
Th. Schuster, T. Kuhn, E.H. Brandt et al., Phys. Rev. B 52,
10 375 共1995兲; 54, 3514 共1996兲; 56, 3413 共1997兲.
10
V.K. Vlasko-Vlasov, G.W. Crabtree, U. Welp, and V.I. Nikitenko

11
J.P. Clerc, G. Giraud, J.M. Laugier, and J.M. Luck, Adv. Phys.
39, 191 共1990兲; M.B. Isichenko, Rev. Mod. Phys. 64, 961

12
A. Gurevich and V.M. Vinokur, Phys. Rev. Lett. 83, 3037 共1999兲.
13
A. Gurevich, Fiz. Tverd. Tela 共Leningrad兲 30, 1384 共1988兲 关Sov.
Phys. Solid State 30, 800 共1988兲兴; Phys. Rev. B 42, R4857

15, 789 共1991兲.
14
J. Straley and S. Kenkel, Phys. Rev. B 29, 6299 共1984兲; E. Hinrichsen, S. Roux, and A. Hansen, Physica C 167, 433 共1990兲;
P.L. Leath and W. Xia, Phys. Rev. B 44, 9619 共1991兲; R.
Haslinger and R. Joynt, ibid. 61, 4206 共2000兲.
15
A. Goyal, E.D. Specht, D.M. Kroeger, and T.A. Manson, Appl.
Phys. Lett. 68, 711 共1996兲; E.D. Specht, A. Goyal, and D.M.
Kroeger, Phys. Rev. B 53, 3585 共1996兲.
16
V.M. Vinokur, M.V. Feigelman, and V.B. Geshkenbein, Phys.
Rev. Lett. 67, 915 共1991兲.
17
E.H. Brandt, Phys. Rev. B 54, 3530 共1996兲; 54, 4246 共1996兲; 55,
14 513 共1997兲; 58, 6506 共1998兲; 58, 6523 共1998兲; 59, 3369

18
C.P. Bean, Rev. Mod. Phys. 36, 31 共1964兲.
19
A.M. Campbell and J.E. Evetts, Adv. Phys. 21, 1191 共1972兲.
20
4025
Th. Schuster, H. Kuhn, and M.V. Indenbom, Phys. Rev. B 52,
15 621 共1995兲.
21
A. Gurevich, Phys. Rev. B 46, 3638 共1992兲.
22
A. Gurevich and J. McDonald, Phys. Rev. Lett. 81, 2546 共1998兲.
23
S.A. Chaplygin, On Gas Jets 共Brown University, Providence, RI,
1944兲; L.I. Sedov, Two-Dimensional Problems in Hydrodynamics and Aerodynamics 共Interscience, New York, 1965兲.
24
L.D. Landau and E.M. Lifshits, Fluid Mechanics 共Pergamon, Oxford, 1987兲; L.M. Milne-Thompson, Theoretical Aerodynamics

25
M. Friesen and A. Gurevich 共unpublished兲.
26
K. Seeger, Semiconductor Physics 共Springer-Verlag, Berlin,
1982兲.
27
W.T. Norris, J. Phys. D 3, 489 共1970兲.
28
J.R. Clem, R.P. Huebener, and D.E. Gallus, J. Low Temp. Phys.
12, 449 共1973兲.
29
E. Zeldov, A.I. Larkin, V.B. Geshkenbein, M. Konczykowski, D.
Mayer, B. Khaykovich, V.M. Vinokur, and H. Shtrikman, Phys.
Rev. Lett. 73, 1428 共1994兲.
30
E. Zeldov, J.R. Clem, M. McElfresh, and M. Darwin, Phys. Rev.
B 49, 9802 共1994兲.
31
E.H. Brandt and M.V. Indenbom, Phys. Rev. B 48, 12 893 共1994兲.
32
L.D. Landau and E.M. Lifshits, Electrodynamics of Continuous
Media, Theoretical Physics Vol. VIII 共Pergamon, Oxford, 1963兲.
33
I.N. Vekua, Generalized Analytical Functions 共Pergamon, London, 1962兲.
34
P.M. Morse and H. Feshbach, Methods of Theoretical Physics

35
Equations 共57兲–共63兲 were obtained for nⰇ1, so they do not reduce to the Ohmic case (n⫽1), described by Eqs. 共51兲 and 共52兲.
However the discrepancy between Eqs. 共57兲–共63兲 and the exact
solution becomes exponentially small for n⬎3, since the accuracy of Eqs. 共57兲–共63兲 is of order exp(⫺␲␤)Ⰶ1. The discrepancy manifests itself as a mismatch of two exact hodograph
solutions ␺ ⫹ (x,y) and ␺ ⫺ (x,y) at the contour E(x,y)⫽E 0 ,
which separates the regions of current flow with E⬎E 0 and E
⬍E 0 , respectively. This mismatch is visible at n⬍3, but becomes undetectable in Figs. 11–16, which correspond to n⬎3.
36
A.V. Gurevich, R.G. Mints, and A.L. Rakhmanov, The Physics of
Composite Superconductors 共Begell House, New York, 1997兲.
37
Handbook of Mathematical Functions, Applied Mathematics Series Vol. 55, edited by M. Abramowitz and I.R. Stegun 共National Bureau of Standards, Washington, DC, 1964兲.
38
X.D. Wu, S.R. Foltyn, P.N. Arendt, W.R. Blumenthal, I.H.
Campbell, J.D. Cotton, J.Y. Coulter, W.L. Hults, M.P. Maley,
H.F. Safar, and J.L. Smith, Appl. Phys. Lett. 67, 2397 共1995兲;
D.P. Norton, A. Goyal, J.D. Budai, D.K. Christen, D.M.
Kroeger, E.O. Specht, Q. He, B. Saffian, M. Paranthaman, C.E.
Klabunde, D.F. Lee, B.C. Sales, and F.A. List, Science 274, 755

39
L.N. Bulaevskii, J.R. Clem, L.I. Glazman, and A.P. Malozemoff,
Phys. Rev. B 45, 2545 共1992兲.
```
Related documents